1 Module 4: Behaviour of a Laminae-II Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties of structure is obtained through the composite micromechanics. Properties the matrix, reinforcement and details of the manufacturing processes a required to obtain information in impact resistance, fracture toughness, uniaxial strength etc. The results usually consist of strength and fracture properties Formal explanation of composite micromechanics in terms of mathematic: models, equations and concepts are based on few assumptions and the principle of solid mechanics. The assumptions include: Ply strengths are associate with their respective fracture modes and there is an intense bond at the, interface between the various constituents. The ply and its constituent resist load and behave linearly elastic to fracture. While the principles of solid mechanics can be used along with various levels of mathematical sophistication, material mechanics is used to derive the equations as it yields explicit equations of simple form for each property. By convention, properties along the fiber directions are called longitudinal properties, the perpendicular ones are called transverse properties, in-plane shear is called intra-laminar shear and those through the thickness are called inter-laminar properties Properties of ply are defined with respect to ply axis for purpose of description or analysis. A letter with suitable subscripts is selected to identify the property. Moisture diffusion through the interfaces of filaments in bulk plastics, and can be represented by equations permitting the extent of damage to the plastics. Load from the matrix are taken by the fiber in shear length. The shear length increases in the direction of the fiber as the load gets transmitted to the fiber. The maximum load is reached when the fiber length is equal to critical length. The possibility of the composite strength reaching that of rule-of-mixtures value occurs when the length of the fiber is greater in relation to the critical length. The constituents of sheet material could be a group of fiber layers bounded together. The composite strength can be fully utilized if tension axis is in the direction of the fibers. The shear strength is weaker when the forces in which the sheet is angled at 90 degrees and the tension applied perpendicular to the fiber orientation that pulls the matrix apart is weak in tension. The angle between the stress application and fiber direction is inversely proportional to the composite strength and least strength is at 45 degrees.
2 The rule-of-mixtures value cannot equal the short length fiber composite theoretically. Practically, however the two values are so close that the difference between them is negligible. The relation between ply uniaxial strengths and constituent properties in a structure is obtained composite micro-mechanics. Note: In this module text in Italic indicates advanced concepts. Assumed Pre-knowledge It is assumed that the student is familiar with simple concepts of mechanical behaviour, such as the broad meanings of stress and strain. It would be an advantage for the student to understand that these are really tensor quantities, although this is by no means essential. All of the terms associated with the assumed pre-knowledge are defined in the glossary, which can be consulted by the student at any time. Composite Material definition: Most composites have strong, stiff fibres in a matrix which is weaker and less stiff. The objective is usually to make a component which is strong and stiff, often with a low density. Commercial material commonly has glass or carbon fibres in matrices based on thermosetting polymers, such as epoxy or polyester resins. Sometimes, thermoplastic polymers may be preferred, since they are mouldable after initial production. There are further classes of composite in which the matrix is a metal or a ceramic. For the most part, these are still in a developmental stage, with problems of high manufacturing costs yet to be overcome. Furthermore, in these composites the reasons for adding the fibres (or, in some cases, particles) are often rather complex; for example, improvements may be sought in creep, wear, fracture toughness, thermal stability, etc. This software package covers simple mechanics concepts of stiffness and strength, which, while applicable to all composites, are often more relevant to fibre-reinforced polymers. M4.1.2 Module Structure The module comprises three sections: Load Transfer Composite Laminates Fracture Behaviour Brief descriptions are given below of the contents of these sections, covering both the main concepts involved and the structure of the software. M Load Transfer Summary
3 This section covers basic ideas concerning the manner in an applied mechanical load is shared between the matrix and the fibres. The treatment starts with the simple case of a composite containing aligned, continuous fibres. This can be represented by the slab model. For loading parallel to the fibre axis, the equal strain condition is imposed, leading to the Rule of Mixtures expression for the Young's modulus. This is followed b y the cases of transverse loading of a continuous fibre composite and axial loading with discontinuous fibres. M Meaning of Load Transfer: The concept of load sharing between the matrix and the reinforcing constituent (fibre) is central to an understanding of the mechanical behaviour of a composite. An external load (force) applied to a composite is partly borne by the matrix and partly by the reinforcement. The load carried by the matrix across a section of the composite is given by the product of the average stress in the matrix and its sectional area. The load carried by the reinforcement is determined similarly. Equating the externally imposed load to the sum of these two contributions, and dividing through by the total sectional area, gives a basic and important equation of composite theory, sometimes termed the "Rule of Averages" which relates the volume-averaged matrix and fibre stresses ( σ m, σ f ), in a composite containing a volume (or sectional area) fraction f of reinforcement, to the applied stress S A. Thus, a certain proportion of an imposed load will be carried by the fibre and the remainder by the matrix. Provided the response of the composite remains elastic, this proportion will be independent of the applied load and it represents an important characteristic of the material. It depends on the volume fraction, shape and orientation of the reinforcement and on the elastic properties of both constituents. The reinforcement may be regarded as acting efficiently if it carries a relatively high proportion of the externally applied load. This can result in higher strength, as well as greater stiffness, because the reinforcement is usually stronger, as well as stiffer, than the matrix. (M ) M What happens when a Composite is stressed? Figure M : loading a composite parallel to the fibres Consider loading a composite parallel to the fibres. Since they are bonded together, both fibre and matrix will stretch by the same amount in this direction, i.e. they will have equal strains, e (Figure M ). This means that, since the fibres are stiffer (have a higher Young modulus, E), they will be carrying a larger stress. This illustrates the concept of load transfer, or load partitioning between matrix and fibre, which is desirable since the fibres are better suited to
4 bear high stresses. By putting the sum of the contributions from each phase equal to the overall load, the Young modulus of the composite is found (diagram). It can be seen that a "Rule of Mixtures" applies. This is sometimes termed the "equal strain" or "Voigt" case. M Transverse Stiffness Also of importance is the response of the composite to a load applied transverse to the fibre direction. The stiffness and strength of the composite are expected to be much lower in this case, since the (weak) matrix is not shielded from carrying stress to the same degree as for axial loading. Prediction of the transverse stiffness of a composite from the elastic properties of the constituents is far more difficult than the axial value. The conventional approach is to assume that the system can again be represented by the "slab model". A lower bound on the stiffness is obtained from the "equal stress" (or "Reuss") assumption shown in Figure M The value is an underestimate, since in practice there are parts of the matrix effectively "in parallel" with the fibres (as in the equal strain model), rather than "in series" as is assumed. Empirical expressions are available which give much better approximations, such as that of Halpin-Tsai. For purposes of comparison, a graph is plotted of equal strain, equal stress and Halpin-Tsai predictions. The Halpin-Tsai expression for transverse stiffness (which is not given in the module, although it is available in the glossary) is: (M ) in which Figure M : Slab model The value of x may be taken as an adjustable parameter, but its magnitude is generally of the order of unity. The expression gives the correct values in the limits of f=0 and f=1 and in general
5 gives good agreement with experiment over the complete range of fibre content. A general conclusion is that the transverse stiffness (and strength) of an aligned composite are poor; this problem is usually countered by making a laminate (see section on "composite laminates"). M Determination of Strength There are several possible approaches to prediction of the strength of a composite. If the stresses in the two constituents are known, as for the long fibre case under axial loading, then these values can be compared with the corresponding strengths to determine whether either will fail. More details about strength are given in the section on "Fracture Behaviour". The treatment is a logical development from the analysis of axial stiffness, with the additional input variable of the ratio between the strengths of fibre and matrix. Such predictions are in practice complicated by uncertainties about in situ strengths, interfacial properties, residual stresses etc. Instead of relying on predictions such as those outlined above, it is often necessary to measure the strength of the composite, usually by loading parallel, transverse and in shear with respect to the fibres. This provides a basis for prediction of whether a component will fail when a given set of stresses is generated (see section on "Fracture Behaviour"), although in reality other factors such as environmental degradation or the effect of failure mode on toughness may require attention. M Working of Short Fibres Short fibres can offer advantages of economy and ease of processing. When the fibres are not long, the equal strain condition no longer holds under axial loading, since the stress in the fibres tends to fall off towards their ends (see Figure M ). This means that the average stress in the matrix must be higher than for the long fibre case. Figure M This lower stress in the fibre and correspondingly higher average stress in the matrix (compared with the long fibre case) will depress both the stiffness and strength of the composite, since the matrix is both weaker and less stiff than the fibres. There is therefore interest in quantifying the change in stress distribution as the fibres are shortened. Several models are in common use, ranging from fairly simple analytical methods to complex numerical packages. The simplest is the so-called "shear lag" model. This is based on the assumption that all of the load transfer
6 from matrix to fibre occurs via shear stresses acting on the cylindrical interface between the two constituents. The build-up of tensile stress in the fibre is related to these shear stresses by applying a force balance to an incremental section of the fibre. It leads to an expression relating the rate of change of the stress in the fibre to the interfacial shear stress at that point and the fibre radius, r. (M ) which may be regarded as the basic shear lag relationship. The stress distribution in the fibre is determined by relating shear strains in the matrix around the fibre to the macroscopic strain of the composite. Some mathematical manipulation leads to a solution for the distribution of stress at a distance x from the mid-point of the fibre which involves hyperbolic trig functions: (M ) where e 1 is the composite strain, s is the fibre aspect ratio (length/diameter) and n is a dimensionless constant given by: (M ) in which n m is the Poisson ratio of the matrix. The variation of interfacial shear stress along the fibre length is derived, according to Equation (M ), by differentiating this equation, to give: (M ) The equation for the stress in the fibre, together with the assumption of a average tensile strain in the matrix equal to that imposed on the composite, can be used to evaluate the composite stiffness. This leads to: (M ) The expression in square brackets is the composite stiffness. The stiffness is a function of fibre aspect ratio, fibre/matrix stiffness ratio and fibre volume fraction. The other point to note about the shear lag model is that it can be used to examine inelastic behaviour. For example, interfacial sliding (when the interfacial shear stress reaches a critical value) or fibre fracture
7 (when the tensile stress in the fibre becomes high enough) can be predicted. As the strain imposed on the composite is increased, sliding spreads along the length of the fibre, with the interfacial shear stress unable to rise above some critical value, t i. If the interfacial shear stress becomes uniform at t i along the length of the fibre, then a critical aspect ratio, s, * can be identified, below which the fibre cannot undergo fracture. This corresponds to the peak (central) fibre stress just attaining its ultimate strength sf, so that, by integrating Equation * (M ) along the fibre half-length: (M ) It follows from this that a distribution of aspect ratios between s and s /2 is expected, if the * * composite is subjected to a large strain. The value of s ranges from over 100, for a polymer * composite with poor interfacial bonding, to about 2-3 for a strong metallic matrix. The effects of changing various parameters on the distributions of interfacial shear stress and fibre tensile stress can be explored and predictions made about whether fibres of the specified aspect ratio can be loaded up enough to cause them to fracture. M Conclusion After completing this section, the student should: Appreciate that the key issue, controlling both stiffness and strength, is the way in which an applied load is shared between fibres and matrix. Understand how the slab model is used to obtain axial and transverse stiffnesses for long fibre composites. Realize why the slab model (equal stress) expression for transverse stiffness is an underestimate and be able to obtain a more accurate estimate by using the Halpin-Tsai equation. Understand broadly why the axial stiffness is lower when the fibres are discontinuous and appreciate the general nature of the stress field under load in this case. Be able to use the shear lag model to predict axial stiffness and to establish whether fibres of a given aspect ratio can be fractured by an applied load. Note that the treatments employed neglect thermal residual stresses, which can in practice be significant in some cases. M Composite Laminates Summary This section covers the advantages of lamination, the factors affecting choice of laminate structure and the approach to prediction of laminate properties. It is first confirmed that, while
8 unidirectional plies can have high axial stiffness and strength, these properties are markedly anisotropic. With a laminate, there is scope for tailoring the properties in different directions within a plane to the requirements of the component. Both elastic and strength properties can be predicted once the stresses on the individual plies have been established. This is done by first studying how the stiffness of a ply depends on the angle between the loading direction and then imposing the condition that all the individual plies in a laminate must exhibit the same strain. The methodology for prediction of the properties of any laminate is thus outlined, although most of the mathematical details are kept in the background. M Laminate Definition High stiffness and strength usually require a high proportion of fibres in the composite. This is achieved by aligning a set of long fibres in a thin sheet (a lamina or ply). However, such material is highly anisotropic, generally being weak and compliant (having a low stiffness) in the transverse direction. Commonly, high strength and stiffness are required in various directions within a plane. The solution is to stack and weld together a number of sheets, each having the fibres oriented in different directions. Such a stack is termed a laminate. An example is shown in the diagram. We already discussed the concept of a laminate, and a pictorial illustration of the way that the stiffness becomes more isotropic as a single ply is made into a cross-ply laminate in introduction section. M Stresses within a Cross-ply Laminate The stiffness of a single ply, in either axial or transverse directions, can easily be calculated. (See the section on Load Transfer). From these values, the stresses in a crossply laminate, when loaded parallel to the fibre direction in one of the plies, can readily be calculated. For example, the slab model can be applied to the two plies in exactly the same way as it was applied in the last section to fibres and matrix. This allows the stiffness of the laminate to be calculated. This gives the strain (experienced by both plies) in the loading direction, and hence the average stress in each ply, for a given applied stress. The stresses in fibre and matrix within each ply can also be found from these average stresses and knowledge of how the load is shared. Note that, particularly with high stiffness ratios, most of the applied load is borne by the fibres in the "parallel" ply (the one with the fibre axis parallel to the loading axis). M Definition Off-Axis Stiffness of a Ply For a general laminate, however, or a crossply loaded in some arbitrary direction, a more systematic approach is needed in order to predict the stiffness and the stress distribution. Firstly, it is necessary to establish the stiffness of a ply oriented so the fibres lie at some arbitrary angle to the stress axis. Secondly, further calculation is needed to find the stiffness of a given stack. Consider first a single ply. The stiffness for any loading angle is evaluated as follows, considering only stresses in the plane of the ply. The applied stress is first transformed to give the components parallel and perpendicular to the fibres. The strains generated in these directions can be calculated from the (known) stiffness of the ply when referred to these axes. Finally, these strains are transformed to values relative to the loading direction, giving the stiffness.
9 Figure M These three operations can be expressed mathematically in tensor equations. Since we are only concerned with stresses and strains within the plane of the ply, only 3 of each (two normal and one shear) are involved. The first step of resolving the applied stresses, sx, sy and t xy, into components parallel and normal to the fibre axis, s 1, s 2 and t 12 (see Figure M ), depends on the angle, f between the loading direction (x) and the fibre axis (1) (M ) where the transformation matrix is given by: 2 c 2 s 2cs T = 2 s 2 c 2cs cs cs c s 2 2 (M ) in which c= cos( f) and c= sin( f). For example, the value of s 1 would be obtained from: (M ) Now, the elastic response of the ply to stresses parallel and normal to the fibre axis is easy to analyze. For example, the axial and transverse Young s moduli (E 1 and E 2 ) could be obtained using the slab model or Halpin-Tsai expressions (see Load Transfer section). Other elastic constants, such as the shear modulus (G 12 ) and Poisson s ratios, are readily calculated in a
10 similar way. The relationship between stresses and resultant strains dictated by these elastic constants is neatly expressed by an equation involving the compliance tensor, S, which for our composite ply has the form: (M ) in which, by inspection of the individual equations, it can be seen that Application of Equation (M ), using the stresses established from Equation (M ), now allows the strains to be established, relative to the 1 and 2 directions. There is a minor complication in applying the final stage of converting these strains so that they refer to the direction of loading ( x and y axes). Because engineering and tensorial shear strains are not quite the same, a slightly different transformation matrix is applicable from that used for stresses (M ) in which, 2 2 c s cs ' 2 2 T = s c cs 2cs 2cs c s 2 2 and the inverse of this matrix is used for conversion in the reverse direction, (M )
11 in which, ' = 2 2 c s cs 2 2 T s c cs 2cs 2cs c s 2 2 The final expression relating applied stresses and resultant strains can therefore be written, (M ) The elements of T, the transformed compliance tensor, are obtained by concatenation (the equivalent of multiplication) of the matrices T ' -1, S and T. The following expressions are obtained (M ) Figure M The final result of this rather tedious derivation is therefore quite straightforward. Equation (M ), together with the elastic constants of the composite when loaded parallel and normal to the fibre axis, allows the elastic deformation of the ply to be predicted for loading at any angle to the fibre axis. This is conveniently done using a simple computer program. As an example, Figure M shows the Young's modulus for the an polyester-50% glass fibre ply
12 as the angle, f between fibre axis and loading direction rises from 0 to 90. A sharp fall is seen as f exceeds about M Obtaining Stiffness of a Laminate Once the elastic response of a single ply loaded at an arbitrary angle has been established, that of a stack bonded together (i.e. a laminate) is quite easy to predict. For example, the Young's modulus in the loading direction is given by an applied normal stress over the resultant normal strain in that direction. This same strain will be experienced by all of the component plies of the laminate. Since every ply now has a known Young's modulus in the loading direction (dependent on its fibre direction), the stress in each one can be expressed in terms of this universal strain. Furthermore, the force (stress times sectional area) represented by the applied stress can also be expressed as the sum of the forces being carried by each ply. This allows the overall Young's modulus of the laminate to be calculated. M Importance of other Elastic Constants There are several points of interest about how a ply changes shape in response to an applied load. For example, the lateral contraction (Poisson ratio, n) behaviour may be important, since in a laminate such contraction may be resisted by other plies, setting up stresses transverse to the applied load. Another point with fibre composites under off-axis loading is that shear strains can arise from tensile stresses (and vice versa). This corresponds to the elements of S which zero in Equation (M ) are becoming non-zero for an arbitrary loading angle (Equation (M ). These so-called "tensile-shear interactions" can be troublesome, since they can set up stresses between individual plies and can cause the laminate to become distorted. The value of S 16, for example, represents the ratio between g 12 and s 1. Its value can be obtained for any specified laminate by using equation M of this section. It will be seen that, depending on the stacking sequence, relatively high distortions of this type can arise. On the other hand, a stacking sequence with a high degree of rotational symmetry can show no tensile-shear interactions. When the tensile-shear interaction terms contributed by the individual laminae all cancel each other out in this way, the laminate is said to be "balanced". Simple crossply and angle-ply laminates are not balanced for a general loading angle, although both will be balanced when loaded at f=0 (i.e. parallel to one of the plies for a cross-ply or equally inclined to the +q and -q plies for the angle-ply case). If the plies vary in thickness, or in the volume fractions or type of fibres they contain, then even a laminate in which the stacking sequence does exhibit the necessary rotational symmetry is prone to tensile-shear distortions and computation is necessary to determine the lay-up sequence required to construct a balanced laminate. The stacking order in which the plies are assembled does not enter into these calculations. M Conclusion After completing this section, the student should: Appreciate that, while individual plies are highly anisotropic, they can be assembled into laminates having a selected set of in-plane properties.
13 Understand broadly how the elastic properties of a laminate, and the partitioning of an applied load between the constituent plies, can be predicted. Be able to use the software package to predict the characteristics of specified laminate structures. Understand the meaning of a "balanced" laminate. M Fracture Behaviour Summary This section covers simple approaches to prediction of the failure of composites from properties of matrix and fibre and from interfacial characteristics. The axial strength of a continuous fibre composite can be predicted from properties of fibre and matrix when tested in isolation. Failures when loaded transversely or in shear relative to the fibre direction, on the other hand, tends to be sensitive to the interfacial strength and must therefore be measured experimentally. An outline is given of how these measured strengths can be used to predict failure of various laminate structures made from the composite concerned. Finally, a brief description is given of what is meant by the toughness (fracture energy) of a material. In composites the most significant contribution to the fracture energy usually comes from fibre pullout. A simple model is presented for prediction of the fracture energy from fibre pullout, depending on fibre aspect ratio, fibre radius and interfacial shear strength. M How do Composites Fracture? Figure M
14 Fracture of long fibre composites tends to occur either normal or parallel to the fibre axis. This is illustrated in Figure M Large tensile stresses parallel to the fibres, s 1, lead to fibre and matrix fracture, with the fracture path normal to the fibre direction. The strength is much lower in the transverse tension and shear modes and the composite fractures on surfaces parallel to the fibre direction when appropriate s 2 or t 12 stresses are applied. In these cases, fracture may occur entirely within the matrix, at the fibre/matrix interface or primarily within the fibre. To predict the strength of a lamina or laminate, values of the failure stresses s 1*, s 2* and t 12* have to be determined. M Prediction of Axial Strength Understanding of failure under an applied tensile stress parallel to the fibres is relatively simple, provided that both constituents behave elastically and fail in a brittle manner. They then experience the same axial strain and hence sustain stresses in the same ratio as their Young's moduli. Two cases can be identified, depending on whether matrix or fibre has the lower strain to failure. These cases are treated in M and M respectively. Figure M Consider first the situation when the matrix fails first (e m* <e f* ). For strains up to e m*, the composite stress is given by the simple rule of mixtures: (M )
15 Above this strain, however, the matrix starts to undergo microcracking and this corresponds with the appearance of a "knee" in the stress-strain curve. The composite subsequently extends with little further increase in the applied stress. As matrix cracking continues, the load is transferred progressively to the fibres. If the strain does not reach e f* during this stage, further extension causes the composite stress to rise and the load is now carried entirely by the fibres. Final fracture occurs when the strain reaches e f*, so that the composite failure stress s 1* is given by f s f*. A case like this is illustrated in Figure M , which refers to steel rods in a concrete matrix. Figure M Alternatively, if the fibres break before matrix cracking has become sufficiently extensive to transfer the entire load to them, then the strength of the composite is given by: (M ) where s is the fibre stress at the onset of matrix cracking (e fm * 1 =e m* ). The composite failure stress depends therefore on the fibre volume fraction in the manner shown in Figure M The fibre volume fraction above which the fibres can sustain a fully transferred load is obtained by setting the expression in Equation (M ) equal to f s f*, leading to: (M )
16 If the fibres have the smaller failure strain, continued straining causes the fibres to break up into progressively shorter lengths and the load to be transferred to the matrix. This continues until all the fibres have aspect ratios below the critical value (see Equation (M )). It is often assumed in simple treatments that only the matrix is bearing any load by the time that break-up of fibres is complete. Subsequent failure then occurs at an applied stress of (1-f) s. If matrix m * fracture takes place while the fibres are still bearing some load, then the composite failure stress is: (M ) where s is the matrix stress at the onset of fibre cracking. In principle, this implies that the mf presence of a small volume fraction of fibres reduces the composite failure stress below that of the unreinforced matrix. This occurs up to a limiting value f ' given by setting the right hand side of Equation (M ) equal to (1-f) s. m * (M ) The values of these parameters can be explored for various systems using M and M Prediction of the values of s 2* and t 12* from properties of the fibre and matrix is virtually impossible, since they are so sensitive to the nature of the fibre-matrix interface. In practice, these strengths have to be measured directly on the composite material concerned. M Failure of Plies under Off-axis Loads Failure of plies subjected to arbitrary (in-plane) stress states can be understood in terms of the three failure mechanisms (with defined values of s 1*, s 2* and t 12* ) which were depicted in introduction. A number of failure criteria have been proposed. The main issue is whether or not the critical stress to trigger one mechanism is affected by the stresses tending to cause the others - i.e. whether there is any interaction between the modes of failure. In the simple maximum stress criterion, it is assumed that failure occurs when a stress parallel or normal to the fibre axis reaches the appropriate critical value, which is when one of the following is satisfied: (M )
17 For any stress system ( sx, syandtxy ) applied to the ply, evaluation of these stresses can be carried out as described in the section on Composite Laminates (Equations (M ) and ( )). Figure M Monitoring of s 1, s 2 and t 12 as the applied stress is increased allows the onset of failure to be identified as the point when one of the inequalities in Equation (M ) is satisfied. Noting
18 the form of T (Equation (M )), and considering applied uni-axial tension, the magnitude of s x necessary to cause failure can be plotted as a function of angle f between stress axis and fibre axis, for each of the three failure modes. (M ) (M ) (M ) The applied stress levels at which these conditions become satisfied can be explored using M As an example, the three curves corresponding to Equations (M )- (M ) are plotted in Figure M , using typical values of s 1*, s 2* and t 12*. Typically, axial failure is expected only for very small loading angles, but the predicted transition from shear to transverse failure may occur anywhere between 20 and 50, depending on the exact values of t 12* and s 2*. In practice, there is likely to be some interaction between the failure modes. For example, shear failure is expected to occur more easily if, in addition to the shear stress, there is also normal tensile stress acting on the shear plane. The most commonly used model taking account of this effect is the Tsai-Hill criterion. This can be expressed mathematically as: (M ) This defines an envelope in stress space: if the stress state (s 1, s 2 and t 12 ) lies outside of this envelope, i.e. if the sum of the terms on the left hand side is equal to or greater than unity, then failure is predicted. The failure mechanism is not specifically identified, although inspection of the relative magnitudes of the terms in Equation (M ) gives an indication of the likely contribution of the three modes. Under uniaxial loading, the Tsai-Hill criterion tends to give rather similar predictions to the Maximum Stress criterion for the strength as a function of loading angle. The predicted values tend to be somewhat lower with the Tsai-Hill criterion, particularly in the mixed mode regimes where both normal and shear stresses are significant. This can be explored in M M Explanation for the Failure Strength of a Laminate The strength of laminates can be predicted by an extension of the above treatment, taking account of the stress distributions in laminates, which were covered in the preceding section.
19 Once these stresses are known (in terms of the applied load), an appropriate failure criterion can be applied and the onset and nature of the failure predicted. Figure M However, failure of an individual ply within a laminate does not necessarily mean that the component is no longer usable, as other plies may be capable of withstanding considerably greater loads without catastrophic failure. Analysis of the behaviour beyond the initial, fully elastic stage is complicated by uncertainties as to the degree to which the damaged plies continue to bear some load. Nevertheless, useful calculations can be made in this regime (although the major interest may be in the avoidance of any damage to the component).in M , a crossply (0/90) laminate is loaded in tension along one of the fibre directions. The stresses acting in each ply, relative to the fibre directions, are monitored as the applied stress is increased. Only transverse or axial tensile failure is possible in either ply, since no shear stresses act on the planes parallel to the fibre directions. The software allows the onset of failure to be predicted for any given composite with specified strength values. Although the parallel ply takes most of the load, it is commonly the transverse ply which fails first, since its strength is usually very low.
20 In M , any specified laminate can be subjected to an imposed stress state and the onset of failure predicted. An example of such a calculation is shown in Figure M M Definition of Toughness (Fracture Energy) of a Composite The fracture energy, G c, of a material is the energy absorbed within it when a crack advances through the section of a specimen by unit area. Potentially the most significant source of fracture work for most fibre composites is interfacial frictional sliding. Depending on the interfacial roughness, contact pressure and sliding distance, this process can absorb large quantities of energy. The case of most interest is pull-out of fibres from their sockets in the matrix. This process is illustrated schematically in M The work done as a crack opens up and fibres are pulled out of their sockets can be calculated in the following way. A simple shear lag approach is used. Provided the fibre aspect ratio, s = L/ r, is less than the critical value, s ( = s /2 t i ) f, see the Load Transfer section, all of the fibres intersected by the crack debond and are subsequently pulled out of their sockets in the matrix (rather than fracturing). Consider a fibre with a remaining embedded length of x being pulled out an increment of distance dx. The associated work is given by the product of the force acting on the fibre and the distance it moves: du = (2prxti*) dx (M ) where t i* is the interfacial shear stress, taken here as constant along the length of the fibre. The work done in pulling this fibre out completely is therefore given by (M ) where x 0 is the embedded length of the fibre concerned on the side of the crack where debonding occurs ( x 0 = L ). The next step is integration over all of the fibres. If there are N fibres per m 2, then there will be ( Ndx / L ) per 0 m2 with an embedded length between x 0 and x + dx ). This allows an expression to be derived for the pull-out work of fracture, G c ( 0 0
21 (M ) The value of N is related to the fibre volume fraction, f, and the fibre radius, r, N f = 12 (M ) r Equation (M4.1.29) therefore simplifies to (M ) This contribution to the overall fracture energy can be large. For example, taking f=0.5, s=50, r=10 µm and t i =20 MPa gives a value of about 80 kj m -2. This is greater than the fracture energy of many metals. Since s f* would typically be about 3 GPa, the critical aspect ratio, s ( s /2t ) f i, for this value of t, would be about 75. Since this is greater than the i actual aspect ratio, pull-out is expected to occur (rather than fibre fracture), so the calculation should be valid. The pull-out energy is greater when the fibres have a larger diameter, assuming that the fibre aspect ratio is the same. The cumulative fracture energy is plotted as the crack opens up and fibres are pulled out of their sockets and the end result for a particular case is shown in Figure M
22 Figure M M Conclusion After completing this section, the student should: Appreciate that a unidirectional composite tends to fracture axially, transversely or in shear relative to the fibre direction. Be able to use simple expressions for axial composite strength, based on fibre and matrix fracturing similarly in the composite and in isolation. Understand what is meant by "mixed mode" failure and be able to use Maximum Stress or Tsai-Hill criteria to predict how a unidirectional composite will fail under multi-axial loading. Be able to use measured strength values for a unidirectional composite to predict how ply damage will develop in a laminate. Understand the concept of the fracture energy of a composite and be able to use the software package to predict the contribution to this from fibre pull-out. M4.1.2 Prediction of Engineering Properties Using Micromechanics Thus far, engineering properties, stiffnesses, compliances, and the relations between them have been discussed without concern for what is happening at the fiber level. While many important issues regarding the response of fiber-reinforced composite materials and structures can be addressed without knowing what is happening at this level, it is often helpful and sometimes
23 even necessary to view composites from this vantage point. The interactions of the elastic properties of the fiber and matrix produce the elastic properties of the composite material. Similarly, the thermal expansion properties of the fiber and matrix interact to produce the thermal expansion properties of the composite. By knowing how the two constituents interact, you can predict the material properties of a composite material. More importantly, by knowing how the two constituents interact, you can design a composite material to achieve particular overall properties. Furthermore, what ultimately determines the load capacity of the composite material is the stress state at this microstructural level, within the matrix, within the fiber, and at the interface between the matrix and fiber. Computing the stresses at this level can be very useful for understanding some of the underlying mechanisms of failure and for constructing failure theories for composite materials. In general, studying the response of a fiber-reinforced composite material at the microstructural level is quite involved. As with viewing composites from the structural level, you must resolve many questions before you can address the response at the micromechanical level. How are the fibers to be represented? How is the matrix to be represented? How many fibers have to be included in the model to properly reflect a representative volume? How are these fibers arranged? Can you assume that the microstructure is repeating or periodic? What length of fiber needs to be considered? Does a fiber have the same properties in its axial direction as across its diameter? What are the material properties of the fiber? How are they determined? After all, it is difficult to load a fiber across its diameter to determine the properties perpendicular to the axial direction. What are the material properties of the matrix? If failure is to be studied, what failure criterion is to be used at that level? From a different viewpoint, what stresses can the fiber withstand? What stresses can the matrix withstand? What stresses can the interface between the fiber and matrix withstand? Is the interphase region, if there is one, important? The need to answer these questions is affected by the type of information being sought by viewing composites from the microstructural level. As this list of questions demonstrates, the issue of micromechanics needs to be viewed carefully, lest the results be misinterpreted. For example, if key information is missing or not known with a high degree of accuracy say material properties of the fiber it may not be worth the effort to study composites at the microstructural level. Nevertheless, because it is important to be versed in the issues, the following sections address issues in micromechanics. After this discussion, we will again focus on the larger scale of a layer of fiber-reinforced material, the so-called macromechanical scale. We hope that the discussion of micromechanics will allow developments in macro-mechanics to be viewed in proper prospective. M Background One of the earliest models of composite materials considered a single infinitely long fiber surrounded by matrix. The matrix surrounding the fiber transfers the load to the fiber. The transfer occurs at the end of the fiber, so one might conclude that an infinitely long fiber is not a good model. However, because the length of most fibers is hundreds of times greater than their diameter, the region of stress transfer into the fiber from the matrix is so small that an infinitelength fiber model can be justified. On the other hand, although the infinitely long approximation may be accurate, the single-fiber model ignores the existence of other fibers near the one being
24 considered. However, the issue in these early models was the overall elastic and thermal expansion properties of the composite, not the details of the stresses or deformations at the microstructural level. As long as the volume of fiber relative to the volume of matrix was represented correctly, the single-fiber model could be justified to some extent. In other views of the microstructure of composites, the fibers were seen as a parallel array of stiff elastic elements joined together by a softer element, the matrix material. A strength-of-materials approach was used to analyze this assemblage of stiff and soft elements. Although such models quite accurately predicted the extensional modulus of the composite in the fiber direction, they were poor predictors of the extensional modulus perpendicular to the fibers. Modifications were introduced to correct these problems, and these modified models have been used with some success. The following sections discuss several kinds of micromechanical models. Results from the various models are presented and comparisons among the models are compared. The primary interest with the models is the prediction of composite material properties. However, to provide insight into failure, we will also discuss stresses in the fiber and matrix. The approach will be to introduce some of the more complex models first. In considering fibers and the surrounding matrix we will assume that the fibers are spaced periodically in square-packed or hexagonalpacked arrays. We will assume that the fibers are infinitely long. To obtain results from these models, numerical approaches must be used. We will present results from the finite-element method and, as will be seen, either the square-packed or hexagonal-packed array model provides a basis for addressing a number of issues related to studying fiber-reinforced composite materials. Though numerical approaches are beyond the scope of this book, we present such results because they provide an accurate representation of response of this level. As a contrast to the numerically based square-and hexagonal-packed array models, we will base the second approach to micromechanics on elasticity solutions. This approach can lead to intractable formulations, but with simplifications results can be obtained. We will use one such simplification, known as the concentric cylinders model, to obtain results for particular problems. As an alternative to the first two approaches discussed, the third series of models discussed will be the simplest. This approach considers the fibers as stiff parallel fiber elements joined by softer matrix material elements. We will analyze these models, referred to as the ruleof-mixtures models, using a strength-of-materials approach. The simplicity and limitations of these models will become immediately obvious. Note: In this module text in Italic indicates advanced concepts. M Finite-Element Results: Square- and Hexagonal Packed Array Models We know that in a fiber-reinforced material, the fibers are distributed throughout the matrix in a pattern we could describe as somewhat repeating or periodic. There is randomness involved, but as a first approximation the cross-section could be idealized as in Figure M (a) or Figure M (b). Figure M (a) illustrates the square-packed array and Figure M (b) illustrates an alternative model, the hexagonal-packed array. The names of the arrays are derived from the shape of the polygons that describe the fiber-packing pattern, and generally the hexagonal-packed array is the preferred model of the two.
25 Figure Cross-section for micromechanics studies If we assume that either of the two models represents to a reasonable degree of accuracy the microstructure of a fiber-reinforced composite material, how can we determine the stresses at the interface between the fiber and the matrix? How can predictions of the fiber-direction extensional modulus be made? What about thermal expansion effects? The first step to obtaining results is to realize that because of the symmetry, only one, or even only part of one, fiber and the surrounding matrix need be considered. If the cross-sections shown in Figure M are representative, then they go on for quite some extent in both cross-sectional directions. (We assumed that the fibers are of infinite length, so the cross-sections of Figure M also go on indefinitely into and out of the plane of the figure.) If, for example, a load is applied in the fiber direction, out of the plane of the figure, then as each fiber is embedded in a vast array of fibers, each fiber will respond the same as its neighboring fibers and attention can focus on a so-called unit cell. Figure M illustrates the concept of a unit cell for both the square-packed and the hexagonal-packed arrays. Because each fiber is embedded in a vast array of other fibers, there is a periodicity to the response, and because of this periodicity, we can argue that the straight lines outlining the unit cells in Figure M (a) and (b) remain straight when the composite is subjected to any one of a number of basic loadings, such as a tensile loading in the fiber direction (in the 1 direction out of the plane of the figure), a transverse tensile loading (from left to right in the 2- direction in the figure), a temperature change, and the like. Because these lines remain straight, attention can be directed at the response of just one unit cell, as in Figure M By directing attention at a unit cell, we easily see that the cross-sectional area of fiber relative to the total cross-sectional area of the unit cell is a measure of the volume of fiber relative to the total volume of the composite. This fraction is an important parameter in composite materials f and is called fiber volume fraction. Fiber volume fraction will be denoted V and it is a number between 0 and 1, usually 0.5 or greater. We will continue to use the coordinate system to study the response of a unit cell. Circumferential locations around the fiber-matrix interface will be identified by the angleθ ; θ will be measured counterclockwise from the 2- axis. Enforcement of the condition that the boundaries of the unit cell remain straight ensures that the isolated unit cell behaves as if it is part of a larger array of unit cells. The disadvantage of these unit cell
26 models is that to obtain results, it is necessary to rely on a finite-element representation of the unit cell. A discussion of the finite-element method of analysis is not possible here, but suffice it to say that a descretization of the cross-section such as that shown in Figure M (a) and (b) is the basis for the method. With the material and geometric symmetry of the coordinate system, depending on the loading, it may actually be sufficient to consider only a portion of the unit cell. Certain symmetry conditions can be enforced along the horizontal and vertical centerlines of the unit cell so that only one-quarter or one-eighth of a unit cell need be modeled. (We will not discuss here the various alternatives that are possible with the modeling.) With a finite-element representation of a unit cell whether it be a full, one-fourth, or one-eighth model it is possible to obtain quite accurate estimates of the response, both of overall response (such as determining E 1 ) and of stresses (such as at the interface between the fiber and the matrix). Figure M Concept of unit cells Figure M Details of Unit cells
27 To follow are results obtained from both the square-packed and the hexagonal-packed models using the quarter-cell finite-element representations in Figure M We present overall elastic and thermal expansion properties of a graphite-reinforced composite, as well as information regarding the stresses in the fiber and matrix. Figure M illustrates the stresses to be discussed, and though they are treated in the context of the square-packed array, these same stresses are definable in the hexagonal-packed array. The normal and shear stresses acting on the interface between the fiber and matrix, σ n andτ ns, have the same value on the matrix side of the interface as on the fiber side. These stress components are responsible for m interface failure in the material. The circumferential stress component in the matrix σ S does not act directly on the interface and does not have the same value as the circumferential stress f component in the fiber, σ S as. The circumferential stress component in the matrix can be responsible for failures originating in the matrix. Finally, we will discuss the stress in the fiber, or 1, direction at the interface. This stress component is not the same in the fiber as it is in the f m matrix. In fact, σ 1 can be responsible for fiber failure, while σ 1 can be responsible for failure of the matrix. These stresses will be studied as a function of angular location,θ around the fibermatrix interface. The direction θ = 0 coincides with the 2-direction, while θ = 90 coincides with the 3-direction. The stresses will also be studied as a function of the fiber volume fraction of the material. The specific values are 0.2, 0.4, and 0.6; the latter is a realistic number, while the two lower numbers are used to provide insight into trends. We should realize that there is an upper bound to fiber volume fraction. The fibers obviously cannot overlap and the upper bound is achieved when all the fibers just touch each other. In addition, we will also study the stresses at the boundaries of the unit cell (see Figure M ). These stresses ( σ 2, σ3,and τ 23) are needed to keep the boundaries of the unit cell straight. Because the analysis assumes that the cross-section represents the infinite length of the fibers, neither stresses nor strains vary along the fiber direction. Such assumptions categorize the analysis as a generalized plane deformation analysis.
28 Figure M Finite-element representations of unit cells (quarter models) Figure Stresses of interest within unit cell M Material Properties of the Fiber and Matrix
29 The elastic and thermal expansion properties of a graphite fiber are taken to be (M ) where the properties are given in the cylindrical coordinate system of the fiber and the superscript f denotes fiber. The above properties correspond to an intermediate-modulus f graphite fiber. The negative value of α x reflects the fact that graphite fibers shrink in the axial direction when heated. Obviously the axial direction (x) of the fiber coincides with the 1- direction. With the above properties, the fiber is said to be transversely isotropic in the r-θ plane (i.e., in the cross-section of the fiber). This means that the fiber responds the same when subjected to a stressσ r, for example, as when it is subjected to stressσ θ. The material in the fiber subjecting to a stress σ x results in a different response. Because of the transverse isotropy, when referred to the coordinate system the fiber properties can be written as (M ) For the polymer matrix material the elastic and thermal expansion properties are taken to be (M ) where the superscript m denotes matrix and the matrix is assumed to be isotropic. All the properties are assumed to be independent of temperature Thermal Effects and Determination of Thermal Expansion Coefficients α 1 and α 2 Always of interest are the stresses at the micromechanical level that result from a temperature change. We can study residual thermally induced stresses due to the cooldown from consolidation by examining the effects of a temperature change. We can also assess the
30 micromechanical stresses due to heating or cooling relative to, say, room temperature. Because the material properties are assumed to be independent of temperature and because thermal expansion is linear with temperature, the micromechanical responses due to a temperature change Δ T basically tell the story. We will present the stresses at the interface between the fiber and matrix and at the boundaries of the unit cell that result from a temperature change Δ T. Because the residual stresses due to cooling from the consolidation temperature are an important issue in composite materials, we will assume the temperature change is negative. For convenience and generality, and with no sacrifice in the physical interpretation of the results, we will normalize the stresses with the quantity E m α m Δ T. This quantity has the units of stress and is the stress in an element of matrix restrained from deforming in one direction. With this normalization the signs of the normalized stresses are the signs that would occur due to cooling from the consolidation temperature. We can easily compute the stresses due to any temperature change by scaling the results by Δ T. To obtain results representing the effects of a temperature change from the finite-element representation of the unit cell of Figure M , the boundary conditions imposed on the finiteelement model are: lines AB, BC, CD, and DA are all free to move and change length but are constrained to remain straight. In reality lines AB, BC, CD, and DA represent surfaces on the sides of the unit cell. Because we assume there are no variations of response in the fiber direction of the unit cell model, the dimension in the fiber direction can be considered unity. Thus, by "free to move," we mean that the net forces acting on the areas represented by the lines AB, BC, CD, and DA are zero. We determine these net forces by the integral of the stresses over the area, with the area being given, for example, by the length of line BC multiplied by 1. More will be said of the integrals of the stresses shortly. In addition to the above stipulations, crosssection ABCD is forced to stay planar and perpendicular to the axis of the fiber during the temperature change, but it may move in the fiber direction. The integral over cross-section ABCD of the normal stresses a\ out of the plane of the figure, namely, the net force in the fiber direction, P, must be zero. Though plane ABCD must remain planar and perpendicular to the fiber axis, it translates in the direction of the fiber axis due to thermal expansion along the fiber direction. The interface normal and shear stresses between the fiber and the matrix for a graphitereinforced material are illustrated in Figure M Results from both the square- and hexagonal-packed arrays are shown. In these and future figures, because of symmetry considerations, the variations of the interface stresses with circumferential location are plotted o only for the range 0 θ 90 o. Also, in general all three fiber volume fractions considered will be on one figure. As Figure M shows, both packing models predict a strong influence of the fiber volume fraction on the interface stress. At 0.2 fiber volume fraction, generally referred to as 20 percent fiber volume fraction, the normal stress σ n is compressive, for the most part independent of circumferential location 0, and has a normalized value of about 0.6. For 20 percent fiber volume fraction the shear stress τ ns is nil. We interpret these results as meaning the fibers that are far enough apart at 20 percent fiber volume fraction that they do not interact (i.e., any particular fiber does not feel the influence of the other fibers in the neighborhood). What occurs at one circumferential location occurs at every other location. As a contrast, at 60 percent fiber volume fraction, the normal stress depends strongly on θ, and there is a shear
31 stress, though it is smaller in magnitude than the normal stress. The square-packed array predicts that the normal stress changes sign with θ, while the hexagonal-packed array predicts the normal stress, while varying with θ, does not change sign and is compressive at all circumferential locations. This strong dependence on θ is to be interpreted as interaction between the fibers, namely, at this volume fraction, the fibers are close enough together that any individual fiber feels the influence of neighboring fibers. Some circumferential locations are closer to neighboring fibers than others and what happens at one circumferential location does not happen at others. For the normal stress the interpretation of the results is as follows: For a negative temperature change and a 20 percent fiber volume fraction, because in the 2-3 planes the matrix material has a larger coefficient of thermal expansion than the fiber, the matrix contracts more and exerts a compressive normal stress on the fiber. Hence, for a negative ΔT the interface normal stresses are compressive, with the value of compressive stress being nearly independent of θ. For 60 percent fiber volume fraction the fibers are closer together, and according to the predictions of the square-packed array, the change in temperature causes tension at the interface in the range 30 < θ < 60. The hexagonal-packed array model predicts variations in the compressive stress as θ varies, but not a tensile stress. For the 60% fiber volume fraction the square-packed array predicts higher compressive stress levels than the hexagonal-packed array, with the high compressive stress levels occurring where the fibers are in closest proximity to one another, such as at θ = 0 and 90 for the square-packed array and θ = 0 and 60 for the hexagonal array. In both models, the shear stress is predicted to change sign and the square array predicts a higher shear stress.
33 Figure M Interface normal and shear stresses in graphite-reinforced material due to a temperature decrease Another stress of interest for the thermally induced case is the circumferential stress (see Figure M ). The circumferential stress in the matrix is, in general, opposite in sign to the circumferential stress in the fiber, though the square-packed array with 60 percent fiber volume fraction predicts a sign change for the fiber stress. The tensile circumferential stress in the matrix is of particular interest. Being tensile and with a severe enough temperature decrease, the stress in the matrix may exceed failure levels and cause the matrix to crack. As a possible scenario, the crack would be oriented radially from the interface into the matrix (see Figure M ). The fiber, on the other hand, is being compressed in the circumferential direction, with no danger of serious fiber failure due to this stress.
34 Figure M Interface circumferential stresses in graphite reinforced material due to a temperature decrease Although they are almost completely independent of circumferential location 0, the stresses in the fiber direction (Figure M ) are important, particularly when interpreted in the context of residual thermal stresses. With the temperature decrease due to cooldown from the consolidation temperature, the stresses in the fiber direction are compressive, while the stresses in the matrix in the fiber direction are tensile. This can be explained as follows: Because the f coefficient of thermal expansion of the fiber in the fiber directionα 1 is negative, as the temperature decreases, the fiber tends to become longer. Conversely, the matrix, with its positive coefficient of thermal expansion, tends to contract in the fiber direction when cooled. Because the fiber and matrix are bonded together, the fiber cannot expand as much as it could if it were free and thus it is in compression in the fiber direction. An extension of the argument leads to the conclusion that the matrix must be in tension. The tensile stress in the matrix could cause matrix cracking to occur. Although it is not shown here, we should mention that in addition to the fact that the fiber-direction stress in the fiber and matrix does not depend strongly on θ, this stress component is tensile and almost uniform within the matrix, and compressive and quite uniform within the fiber. Thus, the fiber-direction stress acting at a point on the cross-section is one of
35 only two different values, the value in the matrix or that in the fiber, depending on where the point is. Figure M Possible crack in matrix due to a temperature decrease Figure M Interface fiber-direction stresses in graphite-reinforced material due to a temperature decrease
36 With the fibers being in close proximity, particularly for the 60 percent volume fraction case, stresses are necessary to keep the unit cell boundaries straight. However, it was also stipulated that there could be no net force on the boundaries of the unit cell. Figure M shows the distribution of the stresses on the boundaries. The important stresses on the boundaries are the normal stresses, σ 2 and σ 3. The shear stresses on the boundaries τ 23 are negligible. In this and other figures illustrating the boundary stresses, the stresses are plotted as a function of normalized distance along the unit cell boundary. The right boundary is represented by line BC (please refer to Figure M ). Due to symmetry, only die upper half of that boundary needs to be considered. Using a normalized distance in the 3-direction, we find that positions on the upper portion of boundary BC for the square-packed array are in the range 0 to 0.5, with 0 coinciding with the 2-axis. Similarly, distances in the 2- direction along the right half of line CD of the square-packed array range from 0 to 0.5, with 0 coinciding with the 3-axis. For the hexagonal-packed array, normalized positions along the upper half of boundary BC range from 0 to 3/2(= 0.867), while normalized positions along the right half of boundary CD range from 0 to 0.5. Note that for the square array the unit cell boundaries are completely in matrix, and for the hexagonal array the unit cell boundaries pass through matrix as well as fiber. The abrupt change in material properties along the boundary lines results in abrupt changes in stress levels. Considering the square array, we find that the normal stresses, 02, along the right boundary, Figure M (a), are compressive near normalized position 0 because the coefficient of thermal expansion of the fiber in the 2-3 plane is less than that of the matrix in that plane. With a temperature decrease, the fiber does not contract as much as the matrix. For line BC to remain straight, a compressive stress is required near 0 to compensate for the lack of fiber contraction. Conversely, because with a temperature decrease the matrix contracts more than the fiber, near position 0.5 tensile stresses are necessary to overcome the greater contraction tendency of the matrix. As the net force along line BC must be zero, the effect of the compressive stresses near position 0 must cancel the effect of the tensile stresses near position 0.5. As an aid to understanding the sign of the stresses along the boundaries of the unit cell, Figure M illustrates the deformations of a unit cell due to a temperature decrease and the greater thermal expansion coefficient of the matrix in the 2-3 plane as compared to the thermal expansion coefficient of the fiber in that plane. Figure M (a) shows the undeformed unit cell before the temperature is decreased, while Figure M (b) shows the deformed unit cell, with the boundaries constrained to remain straight. Figure M (c) shows die deformations that would occur to the unit cell if the boundaries were not constrained to remain straight. The stresses along the boundary BC shown in Figure M (a) and these stresses are necessary for the boundary to remain straight. Due to the symmetry of the thermal problem, the physical interpretation of the stresses along top boundary CD for the square array, Figure M (b), is similar to the interpretation of the stresses along boundary BC. An analogous interpretation of the boundary stresses is possible for the case of the hexagonal array, Figure M (c) and (d).
37 Figure M Stresses on boundaries of unit cell of graphite-reinforced material due to a temperature decrease
38 Figure M Cross-sectional deformations of unit cell of graphite-reinforced material due to a temperature decrease It is not the purpose of this discussion to dwell on the micromechanical-level stresses due to a temperature change. However, from the results just discussed, it is very clear that these stresses can be quite important in determining the integrity of the composite. If there is too large a mismatch between the thermally induced deformations of the fiber and matrix, the stresses can be large enough to cause disbonding of the fiber from the matrix, or cracking in the matrix, or both. Neither of these results can be tolerated. A direct result of the analysis of thermally induced stresses is a determination of the coefficients of thermal expansion of the composite. The change in dimension across the width of the unit cell due to a temperature change provides a measure of the coefficient of thermal expansion transverse to the fiber direction, α 2, while the change in the fiber-direction dimension provides a measure of the coefficient of thermal expansion along the fiber direction, α 1. With either the square-packed or hexagonal-packed array, the coefficient of thermal expansion in the 3- direction, α 3 is equal toα 2. The variations of the coefficients of thermal expansion of the composite with fiber volume fraction are given in Table M , along with other material properties to be discussed shortly. It is readily apparent from the table that the two packing arrays predict nearly identical values of the two coefficients of thermal expansion. Moreover, with increasing volume fraction, the value of 1 α approaches zero and possibly becomes negative, reflecting the increasing influence of the negative coefficient of thermal expansion of the fiber in the fiber direction. In fact, it is seen that for just the right volume fraction of fiber,
39 there would be no thermal expansion of the composite material in the fiber direction, a very useful property and one unique to graphite fiber-reinforced composites. Table M Engineering properties of graphite-reinforced composite Tension in the Fiber Direction and the Determination of Extensional Modulus E 1 and Poisson's Ratios ν 12 and ν13 Because loading in the fiber direction is the loading mode most favorable to composite materials, it is interesting to examine the stresses at the micromechanical level when the composite is subjected to such a load. With the models being used, this loading condition can be simulated by using the same boundary conditions on lines AB, BC, CD, and DA as were enforced for the thermal response case, namely, that those boundaries remain straight and free of any net force. However, instead of having a zero net force on face ABCD, a nonzero value is specified, thus stretching the composite in the fiber direction. The average fiber-direction stress in the composite in the fiber directionσ 1 can then be determined by dividing this specified load, P, by the area of cross-section ABCD, expressed as A. In the figures to follow, the stresses are normalized by this average fiber-direction stress, P/A. As might be suspected, the interface normal and shear stresses, as well as the circumferential stresses in the fiber and matrix at the interface, are minor compared to the fiber-direction stress. Because the case of a fiber-direction loading is a fiberdominated response, and because for the thermal loading the fiber-dominated responses (i.e., α 1 ) of the square-and hexagonal-packed arrays were in such good agreement, only the results from the square-packed array are shown. For 20% fiber volume fraction, the interface normal stress, shown in Figure M , reflects the fact that for a tensile load in the fiber direction, the magnitude of the Poisson effects in the matrix relative to the fiber causes the matrix to compress the fiber in the radial direction. As the fiber volume fraction increases, this clamping effect of the matrix onto the fiber decreases, with
40 o the square array model actually predicting some interface tension near θ = 45 when the fiber volume fraction is 60%. For all volume fractions the interface shear stress is quite small. The circumferential stresses in the matrix, Figure M , also reflect the tendency for the matrix to compress the fiber, with the matrix circumferential stresses causing compression in the fiber as it resists the radial compression effect by trying to push outward on the matrix, something like internal hydrostatic pressure within a void. In turn, the matrix stresses are tensile in the circumferential direction. The most significant stresses for the fiber-direction tensile loading condition are, naturally, the stresses in the fiber direction in the fiber and in the matrix, Figure M It is abundantly clear that while the magnitude of this component of stress depends on the fiber volume fraction, the magnitude is not a function of circumferential location. As in the thermal case (though not shown), for the fiber-direction loading, the fiber-direction stresses in the fiber and matrix are independent of location within the cross-section. We can interpret this as indicating that for this mode of loading, the fibers for this infinitely long unit cell do not interact. Figure M Interfacial normal and shear stresses in graphite-reinforced material due to applied fiber-direction strain, square array Figure M Interfacial circumferential stresses in graphite-reinforced material due to applied fiber-direction strain, square array
41 Figure M Interface fiber-direction stresses in graphite-reinforced material due to applied fiber-direction strain, square array Figure M illustrates the stresses along the boundaries of the square-packed array unit cell that are required for the boundaries to remain straight. Figure M shows the deformations of the cross-section of the unit cell for the case of the boundaries being constrained to remain straight, Figure M (b), and the boundaries being free to deform, Figure M (c). The cross-sectional deformations that occur if the unit cell boundaries are free to deform result m from differences between Poisson's m ratio of the matrix, ν = and Poisson's ratio of the f fiberν xr = Because the matrix has the greater Poisson's ratio, it contracts more in the 2-3 planes than the fiber. It is important to note that although the cross-sectional deformations of Figures and look similar, they each deform the way they do for completely different reasons.
42 Figure M Stresses on boundaries of unit cell of graphite-reinforced material due to applied fiber-direction strain Figure M Cross-sectional deformations of unit cell of graphite-reinforced material due to applied fiber-direction strain We can use the deformations that accompany the fiber-direction tensile loading to compute the fiber-direction extensional modulus and two of the several Poisson's ratios for the composite. The strain in the 2-direction divided by the fiber-direction-1 strain results in one Poisson's ratio, specificallyν 12, while the strain in the 3-direction divided by die fiber-direction strain results in another Poisson's ratio, ν 13, which is identical to ν 12. Table M gives the variations of these composite material properties with fiber volume fraction. The two packing models predict nearly identical results. M Transverse Tensile Loading and Determination of Extensional Modulus E 2 and Poisson's Ratios ν 12 and ν 23 One of the most interesting and important loadings mat can be applied to a fiber-reinforced material is a tensile load or deformation perpendicular to the fiber direction, here the 2- and 3- directions (i.e., the transverse direction). As there is not a continuous path through strong and stiff fiber for the load to be transmitted, the load must either pass through the fiber, across its diameter, through the interface between the fiber and the matrix, through the matrix, through another interface, through another fiber, and so on, or the load must take a somewhat tortuous
43 path, following only matrix material. In reality, a portion of the load follows the matrix-only path and a portion is transmitted through the fiber, with the proportions being determined by the relative stiffness of each constituent and by the fiber volume fraction. With a transverse loading, then, the interaction of fiber and matrix plays a key role in transmitting the stresses through the composite. To study the effects of a transverse load, a known overall transverse strain is imposed on die unit cell model. This is accomplished by stipulating that lines BC and DA in Figure M remain straight and move apart a known amount in the 2-direction, and lines AB and CD are free to move in the 3-direction as long as they remain straight and parallel with the 2-direction. All boundary lines can change length. Additionally, it is specified that cross-section ABCD remains planar and perpendicular to the axis of the fiber. The integral of the fiber-direction stresses acting on that cross-section is again forced to be zero. Figure M indicates the interface normal and shear stresses that result from the transverse strain. Because this is a loading transverse to the fibers, the results from both the square- and hexagonal-packed arrays are shown for comparison. In this and subsequent figures the stresses have been normalized by average transverse stress σ 2 acting along the left and right edges of the unit cell. The average stress is the value required to produce the known transverse strain, and it is determined by integrating the stress σ 2 over boundary BC and dividing by the area of boundary BC. The integrals of these stresses were zero in Figures (a) and (a), cases where the net force in the 2 direction was specified as zero. As expected, the interface normal stress, Figure M , is highest atθ = 0 o, the direction of the imposed transverse normal strain. At the θ = 0 o location the matrix wants to pull away from the fiber because it is transmitting the o transverse load directly to the fiber there. At θ = 90 the square-packed array predicts that the normal stress is compressive, while the hexagonal array predicts that the normal stress there is compressive only for the 20% fiber volume fraction case. In general, the magnitude of the normalized normal stress is, for the most part, independent of fiber volume fraction. It is important to keep in mind that the average transverse stress σ 2 depends on fiber volume fraction. In absolute terms, then, the interface normal stress does depend on fiber volume fraction. The interface shear stress is of significant magnitude, being highest nearθ = 45 o. It is of interest to note that in terms of failure, it may be a combination of the interface tension and the interface shear that causes a problem at the interface. With the variations with θ of the two stress components, it may be that interface failure will not occur where the normal stress is highest, or where the shear stress is highest, but rather at some other circumferential location.
44 Figure M Interfacial normal and shear stresses in graphite-reinforced material due to applied transverse tensile strain With the transverse loading, the circumferential stress, as Figure M shows, is an important component. In Figure M we saw that the interface normal stress is high atθ = 0 o. At this location the transverse tensile stress in the composite is in the direction of the interface normal and the high normal tensile stress was interpreted as the matrix transmitting the o transverse load directly to the fiber. Examination of Figure M shows that also at θ = 90 the matrix transmits the transverse load to the fiber. Atθ = 90 o, for all volume fractions and for both the square- and hexagonal-packed arrays, the circumferential stress in the fiber is much o larger than the circumferential stress in the matrix. At θ = 90 the circumferential direction is aligned with the transverse direction, and it is clear that fiber is taking the majority of the o transverse load. The normal and shear stresses from, say, θ = 45 to θ = 90 o acting in an integrated sense on the fiber-matrix interface, result in the high circumferential stress in the fiber atθ = 90 o. Equilibrium considerations require this high fiber circumferential stress. It should be noted that the hexagonal-packed array shows similar trends in the circumferential stress component, both in the fiber and in the matrix.
45 Figure M Interface circumferential stresses in graphite-reinforced material due to applied transverse tensile strain Figure M shows the fiber-direction stresses at the interface induced in the matrix and fiber. Both the square- and hexagonal-packed arrays predict that the stress in the fiber is, for the most part, independent of circumferential location θ, while the stress in the matrix depends on circumferential location, with the square array showing some sign reversal of the stress in the matrix nearθ = 90 o. With a transverse loading, Poisson effects cause the fiber-reinforced material to contract in the fiber direction. As the fiber is stiff in the 1 direction, it resists and is thus in compression. Because the matrix material is relatively soft, the fiber keeps it from contracting as much as it could and the matrix is, in general, in tension. Because there is no overall force in the fiber direction, the net effect of compressive stresses in the fiber and tensile stresses in the matrix must be zero. While there is little variation of the fiber-direction compressive stress in the fiber within the fiber cross-section there is some variation of the fiber-direction tensile stress within the matrix cross-section.
46 Figure M Interface fiber-direction stresses in graphite-reinforced material due to applied transverse tensile strain Figure M shows the transverse normal stress 2 σ and the shear stress 23 τ acting on the right boundary of the square- and hexagonal-packed unit cells. The shear stresses are inconsequential. The transverse normal stress for the square-packed array, Figure M (a), is largest near position 0 and decreases as position 0.5 is approached. Because the modulus of the fiber in the 2-3-planes is so much larger than the modulus of the matrix, a direct result is that the transverse normal stress is high near position 0.
47 Figure M Stresses on boundaries of unit cell of graphite-reinforced material due to applied transverse tensile strain Along the top boundary of the square array, Figure M (b), the normal stress σ 3 dominates. The average stress along this boundary, which is constrained to remain straight, is zero. Near position 0 a compressive normal stress σ 3 is required, while for positions 0.3 and greater a tensile normal stress is required. The primary reason for this behavior is that in the 2- direction the strain in the matrix is much greater than the strain in the fiber, and through Poisson's ratio there is more contraction strain in the 3-direction in the matrix than in the fiber. For line CD to remain straight the stresses in the 3-direction, Figure M (b), are necessary. A similar interpretation can be given to the more abrupt stress distributions of the hexagonalpacked array, Figure M (c) and (d). We can better understand the stresses on the various boundaries of the square-packed unit cell if we study the deformations associated with the transverse tensile loading, Figure M The average transverse stress, σ 2 as computed from Figure M (a) or (c), divided by the known applied transverse strain is the transverse extensional modulus for the material E 2. The
48 compressive fiber-direction strain, ε 1 divided by the known applied transverse strain, ε 2 and the compressive strain in the other transverse direction, ε 3 both induced by the known applied transverse strain, can be used to determine two Poisson's ratios, ν 21 and ν 23, respectively. As Table M shows, these engineering properties are dependent on the fiber volume fraction. Though the predicted magnitudes of E 2, ν 23 and ν 21 depend somewhat on the packing array used, the predicted trends with fiber volume fraction do not depend on packing array. It is interesting to note from Table M that in spite of the approximations to the microstructure used in these finite-element models, the properties E 1, E 2, ν 12, and ν 21 closely satisfy the reciprocity ν12 ν 21 relation, equation i.e., =. E E 1 2 Figure M toss-sectional deformations of unit cell of graphite-reinforced material due to applied transverse tensile strain M Transverse Shear Loading and Determination of Shear Modulus G 23 Another interesting and extremely important case to examine at the micromechanical level is called the transverse shear response. Transverse shear is used when the unit cell is subjected to a shear stress, or strain, in the 2-3 planes. As with transverse loading, fiber strength and stiffness do not contribute to resisting shear deformation. As a shear response can be decomposed into effective tensile and compressive responses, each oriented at 45 from the direction of shear, the transverse shear loading is somewhat like the transverse tensile loading in that the load must be transmitted partially through the fibers and partially through the matrix; the proportion of load through each constituent depends on the fiber volume fraction and the stiffness of one constituent relative to the other.
49 To study the transverse shear strain response, the outer boundaries of the unit cell are given a displacement that represents subjecting the unit cell to a prescribed overall shear strain. As the square- and hexagonal-packed arrays do not differ substantially in their predictions for the transverse tensile loading case, only the square-packed array will be used to study transverse shear case. The four corners of the unit cell are given displacements in the 2- and 3-directions, and the four boundaries are constrained to remain straight; see Figure M The displacements at each of the four boundaries are similar, and the magnitudes are the same but with differing signs. Plane ABCD is assumed to remain planar and perpendicular to the fiber direction and the integral of the fiber-direction stresses over the area of that plane is required to be zero. There will be stresses along the four boundaries that are necessary to produce the prescribed overall shear strain. Figure M illustrates the interface normal and shear stresses due to the specified overall transverse shear strain as a function of circumferential position around the interface and fiber volume fraction. The stresses have been normalized by the average transverse shear stressτ 23. Although the stresses have been shown only for the range 0 < θ < 90, note that the normal stress is symmetric about θ = 45, while the shear stress is antisymmetric about that location. In Figure M we see that at θ = 45 the normal stress has a maximum tensile value, and that this direction corresponds to the direction of maximum overall tensile strain for the unit cell, that is, from comer A to corner C in Figure M The interface normal stress is zero at θ = 0 and 90 but the at the interface locations the shear stress is maximum. The two stress components have similar magnitudes. Though it appears that neither the normalized interface normal nor the normalized interface shear stress depend strongly on fiber volume fraction, the average shear stress increases with fiber volume fraction. Thus, the absolute level of these interface stresses does depend on fiber volume fraction. Figure M Transverse shear deformations of a square-packed
50 Figure M Interfacial normal and shear stresses in graphite As with the transverse loading, the circumferential stresses in fiber and matrix, Figure M , are important. At θ = 135 (not shown) the circumferential tensile stress in the fiber is a maximum because at this location the softer matrix transfers to the fiber the tensile stress oriented in the 45 direction. That the maximum tensile stress in the fiber occurs at a location 90 from the direction of the effective overall tensile strain is just as it was for the transverse tensile loading case, Figure M (a). There the applied tensile strain oriented in the 2-direction resulted in a maximum tensile stress in the fiber at the 90 location. With the transverse shear case there is the added effective compressive loading aligned with the θ = 135 direction. If the fiber is weak across its diameter, then transverse shear failure may result from the fiber's failing in tension at the 135 location. If the matrix is weak in tension, then failure may occur in the matrix at 45. This assumes that failure has not occurred at the interface due toσ n, orτ ns, or both. The effect of combined tension and compression results in the normalized interface stresses being larger for this transverse shear case than they were for the transverse tension case, though there are analogies between the two loadings. Figure M shows the normalized fiberdirection stresses in the fiber and matrix at the interface region. These stresses reach extreme values at 45. Figure M Interface circumferential stresses in graphite-reinforced material due to applied transverse shear strain, square array
51 Figure M Interface fiber-direction stresses in graphite-reinforced material due to applied transverse shear strain, square array Figure M shows the stresses along the right and top boundaries of the unit cell. The shear stress, τ 23 is not constant along edge BC and a normal stress, σ 2 is required to enforce the deformations of Figure M The magnitudes of the normal and shear stress are similar, but because the normal stress for negative positions in the 3-direction is negative, the average normal stress is zero. As expected, the character of the shear and normal stress along the top edge is stress components along the right edge. The deformations of Figure M can be used to help interpret the character of the stresses along the edges. Figure M Stresses on boundaries of unit cell of graphite-reinforced material due to applied transverse shear strain, square array The average shear stress along the unit cell boundaries, τ 23, determined by the integration of the shear stresses of Figure M , and the known shear deformation of Figure M can be used to determine the transverse shear modulus of the composite, G 23. The variation of this material property with fiber volume fraction is given in Table M ; the value of G 23 increases with fiber volume fraction due to the increasing influence of the fiber. Note, however, that the values ofg 23, ν 23 and E2( E 3) for the square-packed array do not satisfy
52 equation G = E / 2( 1+ ν ) This is because the square array does not lead to transversely isotropic properties even though the constituents are transversely isotropic. The hexagonalpacked array results in transverse isotropy if the constituents are transversely isotropic. The entries for G 23 in Table M for the hexagonal-packed array are computed using equation ( ) G23 = E2 / 2 1+ ν 23. Figure M Cross-sectional deformations of unit cell of graphite-reinforced material due to applied transverse shear strain Note: In this module text in Italic indicates advanced concepts. M Theory of Elasticity Results: Concentric Cylinder Models When fiber-reinforced materials were first used, numerical methods were no readily available as they have become. Therefore, some of the early approaches to studying the response of composite materials at the micromechanics level v based on classical elasticity solutions. Solutions to elasticity problems can be q difficult to determine, and without simplifying assumptions, obtaining solution sometimes impossible. As many of the early elasticity solutions were derived for purpose of determining composite properties from the properties of the constituents as opposed to studying the details of the stresses at, say, the fiber-matrix interface some of the simplifying assumptions were not too limiting. One of the key simplifying
53 assumptions was that the volume of fibers and matrix in a composite a be filled with an assemblage of cylindrical fibers and surrounding matrix mate with the fibers being of various sizes to the degree that the fiber-matrix combination of cylinders completely filled the volume of the composite. This notion is shown in Figure M and is called the composite cylinders model or composite cylinders assemblage. For each fiber-matrix combination, the ratio of the diameter of die fiber to the diameter of the surrounding matrix is the same; this ratio represents the volume fraction of fiber in the composite. For a representative fiber-matrix combination with fiber radius b and matrix outer radius c, the fiber volume fraction is given by (M ) Figure M Philosophy of the concentric cylinders model The elasticity approaches are concentrated on an isolated fiber-matrix combination from this assemblage. Such a combination is shown in Figure M , with the cylindrical x-θ-r and the composite principal material coordinate systems indicated. M Fiber-Direction Tension To study the response of the composite to tension in the fiber direction, we assume that the response of the concentric cylinders is axisymmetric. In addition, if attention is concentrated away from the ends of the fibers, the stresses, and hence the strains, are assumed to be independent of the axial coordinate, namely the x-, or 1-direction. For such conditions, of the three equilibrium equations in cylindrical coordinates, only one is important, and that equation reduces to (M )
54 Figure M Isolated fiber-matrix combination of concentric cylinders model As there are no shear stresses for the axisymmetric axial loading case, the stress-strain relations reduce to (M ) These equations also (inverse relations between stress and strains in the context of the smeared properties of the composite) are also given by the equation as: However, they are equally valid individually for the fiber and for the matrix. Here we will assume that the fiber is transversely isotropic in the r-θ plane and the matrix is isotropic, that is,
55 Thus, the stress-strain relations for the two constituents simplify, for the fiber, to. (M ) and for the matrix, to (M ) where the superscripts / and m denote, respectively, fiber and matrix. Using the engineering properties of the fiber and the matrix, equations (M ) and (M ), and the definitions of the Sij and the Cij -, equations and
56 C, C, C, C, C and C can be computed. f f f f m m , The strains in the above equations are related to the displacements by the strain-displacement relations simplified by the assumptions of axisymmetry and independence of strain of the x- coordinate. There is no shear strain response, only normal strains given by (M ) In equation (M ), u is the axial displacement and w is the radial displacement. Because of the assumption of axisymmetric response, the circumferential displacement, v, is assumed to be zero. Note that the partial derivative of u with respect to x is used and that the ordinary derivative of w ; with respect to r is used because we can argue that w cannot be a function of x, or else the fiber would not be straight when loaded, and at this point in the development, u can be a function of both x and r. Substituting the strain-displacement relations into the stress-strain relations and these, in turn, into equation (M ), which is the third equilibrium equation, leads to an equation for the radial displacement, namely, (M ) which has the solution (M )
57 The quantities A and B are constants of integration that must be solved for by applying boundary and other conditions. The above solution is valid for both the fiber and the matrix. For a given fiber-matrix combination, then, the radial displacement is given by (M a) (M b) where the range of r for each portion of the solution is given. As the strains do not vary with the axial coordinate, the solution for the axial displacement u is given by (M b) (M b) f m where ε1 and ε1 are constants. f According to equation (M a), if B is not zero, the radial displacement at the center of the fiber, r = 0, is predicted to be infinite. This is physically impossible, so the condition (M ) is stipulated. As a result, the strains within the fiber are given by equation (M ) as (M ) while those in the matrix are given by
58 (M ) With the strains defined, the stresses in the fiber and matrix, respectively, can be written as (M a) (M b) When subjected to any loading, in particular an axial load P, the displacements at the interface between the fiber and matrix are continuous; that is, (M ) By substituting expressions for the displacements, equations (M ) and (M ), this condition leads to (M )
59 The second equation leads to the conclusion that the axial strain is the same in the fiber as in the matrix, namely, (M ) This strain is indeed the strain in the composite in the fiber direction, hence the notationε 1, as we have been using all along. As discussed in conjunction with the finite-element results, the radial stress σ r must be the same on the fiber side of the interface as on the matrix side, or (M ) In terms of the unknown constants, substituting for the stresses from equations (M a) and (M b), equation (M ) becomes (M ) At the outer radius of the matrix, if it is assumed that the radial stress must vanish; Using equation ( b), (M ) (M ) As a final condition of the problem, the applied axial load P is actually the integral of the axial stresses over the cross-sectional area of the fiber-matrix combination, namely, (M ) Or
60 (M ) f m If we use equations (M ), (M ), and (M ), the constants A, A, and can be solved for in terms of ε 1. As the early elasticity-based micromechanics analyses were focused on determining overall properties of the composite, in the present case an estimate for f m E 1 can be obtained by substituting the expressions for A and A into equation (M ), resulting in an equation of the form m B (M ) where σ 1 is average stress in the axial, or 1, direction. This is the stress in the composite in the principal material 1 direction and is given by (M ) the axial force divided by the cross-sectional area of the fiber-matrix combination. The expression for t in equation (M ) is complicated but it can be written in the form (M ) The quantities y and 8 are functions of the extensional moduli and Poisson's ratios of the fiber and matrix and the fiber volume fraction. They are given by (M a) and (M b) In the above definitions, as the fiber has been assumed to be transversely isotropic, use has been made of the fact that
61 (M ) For typical properties of the fiber and matrix, γ and δ are much less than one (γ, δ <<1). Hence, to a very good first approximation, E 1 can be written as (M ) f When the major Poisson's ratio of the fiber and Poisson's ratio of the matrix are equal, ν12 = ν both δ and γ are identically zero and equation (M ) is exact. A comparison between the predictions of the finite-element approach and equation (M ) is given in Figure M In the figure, we use equation (M ) to plot the composite extensional modulus, normalized by the modulus of the fiber in the axial direction, as a function of fiber volume fraction. The finite-element» suits from Table M are indicated at the volume fractions studied in that approach. As can be seen, the comparison is excellent. If equation (M ) had been used in. stead of equation (M ), it would have been impossible to detect the difference Figure M Thus equation (M ) can be considered an accurate equation for determining E. 1 Even though the presence of other fibers encourages us to say that the axisymmetric assumption is invalid, it is interesting to compute the stresses predicted by the fiber-matrix cylinder model and compare them with the stresses computed by the finite-element model. The finite-element model, of course, was not restricted by the assumption of axisymmetry and the comparisons are shown in Figures In these figures the various stress components at the fibermatrix interface are plotted as a function of circumferential location around the interface. The finite-element calculations are taken from Figures The finite-element calculations for the hexagonal array, though not included in Figures , are added to Figures Examination of Figure M reveals that for a 20% fiber volume fraction, the axisymmetric assumption of the concentric cylinders model is a good approximation. None of the major stress components vary greatly with θ and the concentric cylinders model provides a good indication of the average level of stress. The interfacial shear stress τ ns varies but its value is quite small compared to the interfacial normal stress σ n. With a 20% fiber volume fraction it would appear that the fibers are far enough apart that they act independently of each other when subjected to an axial load. When the fiber volume fraction is 40%, Figure M , the m f assumption of axisymmetry appears to be less valid, though for the stress componentsσ s, σ 1, m
62 m and σ 1 the assumption appears quite valid. For the other stress components, the comparison of the elasticity solution with the hexagonal-packed array is still quite reasonable; the interfacial shear stress τ ns exhibits the poorest comparison, although it is not a major stress component. For a 60% fiber volume fraction comparison between the elasticity solution and either the square- or hexagonal-packed array finite-element calculations indicate that for the stress components σ n, τ ns, andσ f s, the axisymmetric assumption is not particularly good. However, m f m forσ s, σ 1, and σ 1 the assumption of axisymmetry provides a good estimate of the stresses. Despite the lack of perfect correlation between the stress predictions of the elasticity solution and the finite-element calculations, the prediction of E 1 is obviously not influenced by these errors. The prediction of E 1, a property that can be considered an averaged quantity, really depends on the stresses being accurately predicted in an average sense. The axisymmetric elasticity model does predict the average value of the stresses very well; the variations with θ are not accurately predicted for the higher volume fractions. Figure M Variation of composite modulus E 1 with fiber volume fraction for graphitereinforced material, concentric cylinders model
63 Figure M Comparison of stresses between concentric cylinders model elasticity solution and finite-element calculations for graphite-reinforced material, fiber-direction loading and 20% fiber volume fraction
64 Figure M Comparison of stresses between concentric cylinders model elasticity solution and finite-element calculations for graphite-reinforced material, fiber-direction loading and 40 percent fiber volume fraction
65 Figure M Comparison of stresses between concentric cylinders model elasticity solution and finite-element calculations for graphite-reinforced material, fiber-direction loading and 60 percent fiber volume fraction M Axial Shear
66 The elasticity approach can also be used to estimate values of the shear modulusg 12 ; this modulus is often referred to as the axial shear modulus. The approach to this problem is based on a slightly different view of the fiber-matrix combination, namely, that of Figure M Figure M Axial shear deformation applied to concentric cylinders model In this figure the fiber-matrix combination is viewed by looking along the 3-axis toward the 1-2 plane and die boundaries of the fiber-matrix combination are deformed by shearing in the 1-2 plane. The boundaries of the portion of the fiber-matrix combination shown have the following displacements relative to the undeformed state: (M ) where x1, x 2, and x 3, are used to denote the coordinates in the principal material directions, u1, u2and u3 are the displacements in those directions. The quantity y 2 is the shear strain imposed on the boundary. Though equation (M ) defines a fairly specific deformation on the boundary, in the interior of the fiber-matrix combination the displacements are assumed to be expressible as (M )
67 The function φ ( x, x ) 2 3 defines the shear strains in the interior of the fiber-matrix combination, with the particular form of equation (M ) leading to relatively simple expressions for the shear strains, namely, (M ) It is important to note that there is a function φ for the fiber region and a different function φ for the matrix region. As the other strains are zero, the only stresses present in the fiber-matrix combination due to the displacements given in equation (M ) are (M ) or if we use equation (M ), (M ) where it has been assumed that the material is either isotropic or transversely isotropic, namely, (M ) Because all the stresses except τ 12 and τ 13 are zero, the equilibrium conditions reduce to (M ) Using equation (M ) in equation (M ) results in
68 (M ) and at this point it is convenient to express the problem in cylindrical coordinates; the principal material coordinate system (1-2-3) and the cylindrical coordinate system (x-r-θ) are shown in Figure M Relations between the coordinates in the two systems are given by (M a) and the inverse (M b) The nonzero stresses in the cylindrical coordinate system are related to τ 12 and τ 13 by (M a) and the inverse relations (M b) In terms ofφ, the two shear stresses in the cylindrical coordinate system are
69 (M ) Figure M The x-y-z and coordinate systems for the fiber-matrix combination Writing equation ( ) in the cylindrical coordinate system results in (M ) Equations (M ) and (M ) are Laplace's equation for φ in the two different coordinate systems. The separation of variables technique can be used to solve equation (M ); the solution is given by (M ) For the problem here, only terms to n = 1 are necessary. Additionally, a 0 = 0 and the sin ( nθ ) terms are not needed. Finally, for the stresses to remain bounded at the center of the fiber, B n for the fiber must be zero. As with past practice, using superscripts f to denote the fiber and m to denote the matrix, the functions φ for these two materials in the fiber-matrix combination are
70 (M ) and (M ) As a result, (M ) and (M ) Continuity of the three components of displacement at the interface between the fiber and matrix reduces to enforcement of (M ) or (M ) where, recall, b is the radius of the fiber. Continuity of the stresses at the fiber-matrix interface reduces to a single condition, namely,
71 (M ) which from equations (M ) and (M ) can be written as (M ) Using equation (M ) to enforce the conditions of equation (M ) at the boundary of the fiber-matrix combination (i.e., at r = c and θ = 0), provides a final condition that can be written as (M ) Substitution from equation (M ) yields (M ) f and solving equations (M ), (M ), and (M ) leads to the solution for a1, a 1 m and b 1, namely, m (M ) Accordingly, using equation (M ) in the transformation relations, equation (M b), leads to
72 (M ) m m Evaluating this at r = c and θ = 0 and substituting for a 1 and b 1 from above leads to the following relation between τ 12 andγ o 12 : (M ) This is an important expression because it provides an estimate of the composite axial shear modulus G 12 through the relation (M ) Specifically, (M ) The dependence of 12 G on fiber volume fraction for the graphite-reinforced material is illustrated in Figure M As the fiber volume fraction increases toward 65%, the shear stiffness of the fiber produces about a factor of three increases in the shear stiffness of the composite relative to the matrix, a trend seen with the other composite elastic properties.
73 Figure M Variation of composite axial shear modulus G 12 with fiber volume fraction for graphite-reinforced material, concentric cylinders model M Strength-of-Material Results An important result that can be obtained from the concept of the unit cell and the use of finite elements, or the use of elasticity solutions, is an estimate of the overall elastic and thermal expansion properties of the composite. With these models it is possible to evaluate how the overall properties are influenced by fiber volume fraction, fiber properties, matrix properties, and the assumptions of how the fibers are packed (i.e., square- or hexagonal-packed arrays). While the use of finite-element representations of unit cells provides detailed information about the stresses in the fibers, in the matrix, and at the interface between the fiber and matrix, often it is only the elastic or thermal expansion property estimates that are of interest. This was the case in early micromechanics studies, whereby strength-of-materials approaches were used to provide insight into the elastic properties. These approaches can be considered to be at the opposite end of the spectrum from the finite-element or elasticity approaches. The strength-of-materials approaches do not concern themselves with the details of the stresses at the fiber-matrix interface, the packing arrangements, or the many other characteristics that can be considered with unit cell finite-element models. However, reasonable estimates of some of the elastic and thermal expansion properties of composite materials can be obtained with these approaches. They shall be studied next to provide a contrast to the unit cell finite-element methods. In addition, the strength-of-materials approaches result in rather simple algebraic expressions for the elastic and thermal expansion properties of the composite as a function of fiber and matrix properties. These algebraic expressions can be conveniently used for parametric studies or for embedding within other analyses. M Model for E 1 and ν 12
74 The strength-of-materials models, sometimes called rule-of-mixtures models, also rely on what could be termed a unit cell. The unit cell used in the strength-of-materials models is quite different from the unit cells of the previous sections, and the particular unit cell considered depends on the composite property being studied. To study E 1 and ν 12 for the composite, consider a section cut from a single layer of fiber-reinforced material. The section consists of side-by-side alternating regions of fiber and matrix, the fibers arranged in parallel arrays, as in f Figure M , the widths of each of the regions of fiber and matrix denoted by W and W m, respectively. The figure shows the 1 and 2 principal material directions. The thickness of the layer is not important at the moment, and can be taken as unity. In fact, in these rule-of-mixtures models the cross-sectional shape of the fibers is not important. They can be considered circular, square, elliptical, or any other shape. For simplicity, assume they are square. As it will turn out, only the cross-sectional areas of the fiber and matrix will be important. Figure M (a) shows details of a "unit cell" cut from a single layer, the length of the cell denoted by L and the cross-sectional areas of the fiber and matrix denoted as A f and A m. Assume as in Figure M (b) that the unit cell is subjected to a stress σ 1 such that it stretches in the 1 direction and, due to Poisson effects, contracts in the 2 direction. Because the fiber and matrix are bonded together, they both stretch the same amount in the 1 direction, namely Δ L ; the strain in the 1 direction in both the fiber and matrix is given by (M ) Figure M Section cut from a fiber-reinforced composite and a unit cell
75 Figure M Details of unit cell and rule-of-mixtures model for composite extensional modulus E 1 and major Poisson's ratio ν 12 Because the fiber and matrix have different Poisson's ratios, they will not contract the same amount in the widthwise, or 2, direction. The combined contraction of the fiber and matrix results in the overall contraction of the composite in the 2 direction. That will be addressed shortly. Treating the two constituents as if they were each in a one-dimensional state of stress, we find the stresses in the fiber and matrix are (M ) and accordingly the forces in the 1 direction in the fiber and matrix are given by
76 (M ) The total force in the 1 direction divided by the total cross-sectional area of the unit cell, A, f m where A= A + A, is defined as the composite stressσ 1, namely, (M ) But ΔL is the composite strain ε 1, equation (M ) gives L (M ) where (M ) f m with the quantities V and V being the area fractions of fiber and matrix, respectively. By the f m geometry of the unit cell, however, V and V represent volume fractions. Because (M ) equation (M ) can be written as (M ) Note that this equation is identical to equation (M ), the approximation to the prediction of E 1.From the elasticity model; the exact prediction is given by equation (M ). Thus, the strength-of-materials and elasticity solution predictions are closely related. Equation (M ) is referred to as the rule-of-mixtures equation for E 1.
77 As a summary of all the results obtained, Figure M shows the composite fiber direction modulus, E 1, as a function of fiber volume fraction for a graphite-reinforced material as predicted by the rule of mixtures, the two finite-element arrays, and the exact expression from the theory of elasticity, which use the material properties from equations (M ) and (M ). The relation is obviously linear and clearly the simple rule-of-mixtures model is quite accurate; the differences among the various approaches are indistinguishable. The overall contraction of the unit cell in the 2 direction can be used to compute the major Poisson's ratio of the composite, specificallyν 12. For the situation in Figure M (b), because the unit cell is being subjected to a simple uniaxial stress state, ν 12 is defined as minus the ratio of the contraction strain in the 2 direction divided by the elongation strain in the 1 direction, namely, (M ) Figure M Rule-of-mixtures prediction for variation of composite modulus i with fiber volume fraction for graphite-reinforced material From Figure M , (M )
78 and (M ) Using the definition of Poisson's ratio for each constituent and the fact that each constituent is assumed to be in a state of uniaxial stress, we find the contraction of each constituent is (M ) or (M ) Substituting these relations into equation (M ) and dividing both sides by W results in (M ) The fiber and matrix volume fractions can be identified, and as a result, equation (M ) becomes (M ) From the definition of Poisson's ratio in equation (M ), (M ).
79 or using equation (M ), we find (M ) This is the rule-of-mixtures expression for the major Poisson's ratioν 12. It is very similar to the rule-of-mixtures expression for the modulus E 1 in that it is linear in all of the variables. f Figure M shows the variation of ν 12 with fiber volume fraction for a graphite-reinforced composite, and a comparison of equation (M ) with the finite-element results. Again, the accuracy of the simple rule-of-mixtures results for ν 12 is quite obvious and it is similar to the accuracy of the results for E 1. If interest centers only on knowing E 1 andν 12, then there is really no reason for using the finite-element approach, as the rule-of-mixtures equations are very accurate. As noted before, the derivations and results are independent of the geometry of the fiber or matrix cross-section, an interesting finding in itself. Figure M Rule-of-mixtures prediction for variation of composite major Poisson's ratio ν with fiber volume fraction for graphite-reinforced material 12 M Models for E 2 We can approach one of the most basic considerations for the determination of E 2 by studying the unit cell of Figure M when it is subjected to a transverse stress, σ 2 as in Figure M Isolating the fiber and matrix elements, we can argue by equilibrium that each
80 element is subjected to the same transverse stress, σ 2. If this is the case, then the transverse strain in the fiber and matrix are, respectively, (M ) Considering again a one-dimensional stress state, we find the stress and strain in the fiber and matrix are related by (M ) These equations can be rearranged and written as (M ) The overall change in the transverse dimension of the unit cell is (M )
81 Figure M Rule-of-mixtures model for composite extensional modulus E 2 so the definition of overall transverse strain is (M ) Using equation (M ) in equation (M ), we find (M ) Using the definitions of the fiber and matrix volume fractions and the geometry of the unit cell yields (M )
82 Comparing the above equation with the form (M ) where E 2 is the composite transverse modulus, we see that (M ) or (M ) This equation is the rule-of-mixtures relation for the transverse modulus as a function of the transverse moduli of the fiber and matrix, and the fiber volume fraction. Like rule-of-mixtures relations for E 1 andν 12, this relation is a simple linear relation, in this case among the inverse moduli and volume fractions of the two constituents. Figure M illustrates the comparison between the above rule-of-mixtures expression and the results from the finite-element unit cell model. The rule-of-mixtures expression for E 2 is not in the good agreement with the finiteelement results seen with E1 andν 12. Perhaps this could be expected from the onset, as the freebody diagrams of the fiber and matrix elements in Figure M are something of an oversimplification of the interaction between the fiber and the matrix when the composite is subjected to a transverse stress. For one thing, the one-dimensional state of stress may not be accurate because, like the situation depicted in Figure M , the fiber and matrix elements are bonded together and hence change length together in the 1 direction. Considering the onedimensional stress state, we find the diagram of Figure M indicates that due to the different Poisson's ratios, the element of fiber is allowed to contract in the 1 direction differently than the element of matrix. Thus, a modification of the model would be to have the length change in the 1 direction of the fiber element and the matrix element is the same, an approach to be taken shortly. However, another difficulty with the simplification of Figure M is the diagram assumes that both the fiber and matrix are subjected to transverse stressσ 2. The finiteelement unit cell models demonstrated that a portion of the transverse stress is transmitted through the fiber, and a portion is transmitted around the fiber, through the matrix material. To use a specific nomenclature, the transverse stress σ 2 in the fiber and matrix is partitioned differently than is implied by Figure M To correct the rule-of-mixtures model for 2 E, a so-called stress-partitioning factor is often introduced into equation (M ) to account for
83 the error in the assumption that both the fiber and the matrix are subjected to the full valueσ 2. The stress-partitioning factor accounts for a more proper division of the stress in each of the two constituents. To incorporate a partitioning factor, consider equation (M ) rewritten in slightly different form, specifically, (M ) Figure M Rule-of-mixtures prediction for variation of composite modulus E 2 with fiber volume fraction for graphite-reinforced material Dividing the numerator and denominator by W and again using the geometry of the unit cell as it relates to the fiber and matrix volume fractions, we find equation (M ) becomes
84 (M ) m Now consider that instead of V being the volume fraction of matrix that is subjected to stress m level σ 2, assume the volume fraction is less than that, namely, η V, where η will be referred to as a partitioning factor and 0 < η < 1. The volume fraction of fiber that is subjected to stress f level σ 2 is stillv. As a result of this new nomenclature, the total effective volume of fiber and matrix is now (M ) Equation (M ) now takes the form (M ) and by analogy with equation (M ), the composite modulus E 2 is given as (M ) or (M ) This expression for E 2 is referred to as the modified rule-of-mixtures model forη. The stresspartitioning factor η generally must be determined empirically. If it can be determined for a specific material by measuring E 2 at a particular volume fraction, and if the elastic properties of
85 the fiber and matrix are known, then the value of η can be determined and used for parameter studies involving other fiber volume fractions. Note that when η = 1 in equation (M ), the original rule-of-mixtures relation, equation (M ), is recovered. Figure M illustrates the predictions of the modified rule-of-mixtures model for E 2 as a function of fiber volume fraction, where three values of the stress partitioning factor η are used for purposes of the example. The finite-element results for both square- and hexagonal-packed arrays are used for comparison. A value of η = 0.4 gives a good comparison with the squarepacked array, while a value of η = 0.5 gives a good comparison with the hexagonal-packed array. As mentioned previously, the rule-of-mixtures model for E 2 violates intuition regarding the response of the fiber and matrix elements in that the fiber element is allowed to change length independently of the change in length of the matrix element. Figure M can be modified to account for the elements changing length by the same amount when subjected to a transverse stressσ 2. This will imply, of course, that each element is subjected to a stress in the 1 direction, σ 1. The free-body diagrams of the elements with the two stress components are shown in Figure M , and the deformed transverse widths of the fiber and matrix elements are, respectively, (M ) while the deformed length of both elements is (M ) Considering each element to be in a state of stress such that (M )
86 Figure M Modified rule-of-mixtures prediction for variation of composite modulus E 2 fiber volume fraction for graphite-reinforced material Figure M Alternative rule-of-mixtures model for composite extensional modulus E 1 we find the stress-strain relations for the fiber element are (M a) while for the matrix element,
87 (M b) In the above (M a) and (M b) Using the assumptions given by equation (M ) for both the fiber and the matrix, equations (M a) and (M b) are derivable from either equation or equation
88 Due to equilibrium considerations (M ) and more importantly (M ) This latter equation results from the fact there should be no net force in the 1 direction when the composite is subjected to a transverse stress. If we assume that the stress in the 1 direction is constant within the fiber element, and also within the matrix element, then the condition given in equation (M ) can be written as (M ) Also, because of the geometry of the deformation, (M ) Using equations (M ) and (M ) in the stress-strain relations equations (M a) and (M b), as well as using equation (M ), results in equations that f m can be used to find ΔW and Δ W, and ultimately E 2. With some rearrangement these equations are
89 (M ) f m Solving for ΔW and Δ W and using the basic definition of e2, namely equation (M ), results in a relation of the form (M ) Dividing by σ yields the expression for E 2, namely, (M ) or (M ) To arrive at equation (M ), we've made use of the fact that for the geometry of Figure f m f m M , A and A are directly related to the volume fractions V and V, respectively. Also, the fiber and matrix partitioning factors are given by
90 (M ) Equation (M ) is an alternative version of the rule of mixtures. Figure M shows comparison of results from the alternative rule-of-mixtures model with the results from the finite-element and rule-of-mixtures models. Relative to the rule-of-mixtures model, there is some improvement in the comparison with the finite-element models. Assuming the empirically derived stress-partitioning factor η is known, we find the modified rule-of-mixtures model of equation (M ) appears to be most accurate for the incorporation of a simple formula into a parameter study. However, if an empirically derived stress-partitioning factor is not available, the alternative rule-of-mixtures model can be used for improved accuracy relative to the rule-ofmixtures model, and there is a physical basis for the model. Figure M Alternative rule-of-mixtures prediction for variation of composite modulus 2 with fiber volume fraction for graphite-reinforced material Model for G 12
91 The rule-of-mixtures model for the axial, or fiber-direction, shear modulus G 12 is similar to the rule-of-mixtures model for E 2. The fiber and matrix elements are each considered to be subjected to shear stressτ 12, as in Figure M By equilibrium considerations, the shear stress on the fiber element has to be the same as the shear stress on the matrix element, and thus the shear strains in the elements of fiber and matrix in Figure M are given by Figure M Rule-of-mixtures model for composite axial shear modulus G 12 (M a) (M a)
92 f m where the shear modulus in the fiber and matrix are given by, respectively, G 12 and G. By the geometry of the deformation and the definition of shear strain, (M a) (M b) By considering the fiber and matrix elements joined together, as in Figure M (c), the total deformation of the unit cell is (M ) The average shear strain for the unit cell is then (M ) Substituting equation (M ) into equation (M ), we find (M ) or, if we use equation (M ), (M ) Substituting the stress-strain relations, equation (M ), and recognizing the definition of the volume fractions, we find equation (M ) becomes (M ) By analogy,
93 (M ) G 12 being the axial shear modulus of the composite, and from equation (M ), (M ) OR (M ) This is the rule-of-mixtures expression for G 12. Figure M illustrates the relationship between G 12 and fiber volume fraction for the rule-of-mixtures model; die concentric cylinder model elasticity solution prediction, equation (M ), is shown for comparison. The comparison is not good, as the rule-of-mixtures model generally underpredicts the shear modulus.
94 Figure M Rule-of-mixtures prediction for variation of composite axial shear modulus G with fiber volume fraction for graphite-reinforced material 12 As with the transverse modulus, E 2, we can modify the partitioning assumption for the shear stress in the fiber and matrix and develop a modified rule-of-mixtures model for G 12, resulting in (M ) where η ' is the partitioning factor for the shear stresses. Figure M shows the variation of G 12 as predicted by the modified rule-of-mixtures model with η ' = 0.6, along with the elasticity solution predictions; the value of η ' = 0.6 leads to good correlation with the elasticity solution Model for α 1 and α 2 The rule-of-mixtures model for the coefficients of thermal expansion in the fiber and transverse directions α 1 and α 2 is similar to the alternative rule-of-mixtures model for the transverse modulus E2 in that interaction between the fiber and matrix elements must be accounted for.
95 Referring again to Figure M and considering spatially uniform thermal expansion effects, we find the stress-strain relations for the fiber element are, by analogy with equation (M a), (M a) Figure M Modified rule-of-mixtures prediction for variation of composite axial shear modulus G 12 with fiber volume fraction for graphite-reinforced material while the stress-strain relations for the matrix element are (M b) Equations (M a) and (M b) are derivable from equation
96 or (M d) The relations of equation (M ) remain valid, and the coefficients of thermal expansion of the fiber in the 1 and 2 directions and the coefficient of thermal expansion in the matrix are given f f byα 1, α 2, andα m, respectively. The temperature change relative to some reference level is Δ T. Because fiber and matrix elements are bonded together and therefore must change length the same amount in the 1 direction, (M ) As with past derivations (M ) By equilibrium,
97 (M ) and for the case of imposing a temperature change with no force applied in the 2 direction 0 (M ) resulting in (M ) Likewise, for no applied force in the 1 direction, as in equation (M ), (M ) or, again assuming the stress σ 1 is constant within each constituent, we find that (M ) Thus, from equations (M ) and (M ) and the stress-strain relations given by equations (M a) and (M b), (M )
98 (M ) f f m m Solving this set of equations leads to expressions for ΔW / W, Δ W / W, and Δ L / L. By definition, for no applied loads, the strain in the 1 direction per unit temperature change is the coefficient of thermal expansion in the 1 direction; that is, (M ) Substituting the solution for Δ L / L from equation (M ) into equation (M ) leads to a relation between α 1 and volume fraction, namely, (M ) or (M ) The total change in width of the unit cell due to a temperature change is (M ) Dividing by the total width of the unit cell, and using a slight rearrangement of terms, we find (M ) Recognizing the definitions of volume fraction, we find this equation becomes
99 (M ) Again by definition, the coefficient of thermal expansion in the 2 direction is, for the case of no applied loads, the strain in the 2 direction per unit temperature change; that is, (M ) or (M ) f f m m Substituting the solutions for ΔW / W and Δ W / W from solving equation (M ) into equation (M ) provides a relation for a2 as a function of volume fraction, specifically, (M ) where the rule-of-mixtures composite modulus E 1 has been used to simplify the expression for α 2. Note that a simple rule-of-mixtures model for α 2 would lead to (M ) This simple model would not enforce the fact that the change in length in the 1 direction of the fiber and matrix elements must be the same. The additional terms in equation (M ) relative to equation (M ) reflect the effect of this geometric constraint. Equation (M ) can be written as
100 (M ) while equation (M ) can be written as (M ) Both equation (M ) and equation (M ) express α 2 as a function of fiber volume fraction. It should be noted that a simple rule-of-mixtures expression for α 1 does not make sense, as it is clear the matrix and fiber must expand the same amount in the 1 direction when the temperature is changed. The simple rule-of-mixtures model in the fiber direction, as has been seen, ignores this fact. The relation between the fiber volume fraction and the coefficient of thermal expansionα 1, equation (M ), is shown in Figure M The results given by equation (M ) agree well with the finite-element predictions and hence the equation can be considered useful for determining α 1. Note that for fiber volume fractions greater than 0.6, α 1 is predicted to be negative, reflecting the dominance of the negative value of the fiber expansion f in the 1 direction, α 1.
101 Figure M Rule-of-mixtures prediction for variation of composite coefficient of thermal expansion α 1 with fiber volume fraction for graphite-reinforced material The predictions for the coefficient of thermal expansion 2 α given by equation (M ) and the simpler rule-of-mixtures equation (M ) are shown in Figure M The more complex relation, equation (M ), which reflects interaction between the fiber and matrix, more closely matches the predictions of the square and hexagonal arrays, indicating that the constraint effects represented by the more complicated alternative equation are important.
102 Figure M Rule-of-mixtures prediction for variation of composite coefficient of thermal expansion α 2 with fiber volume fraction for graphite-reinforced material Summary This completes the discussion of micromechanics, an involved, important, and interesting view of fiber-reinforced composite materials, a view that can require a great deal of specialization. Several approaches have been presented for studying micromechanics, the approaches depending to a large degree on the information being sought. Most important for the remainder of this book is the fact that this short study of micromechanics has provided estimates of the elastic and thermal expansion properties that are needed to study the response of composite laminates. To that end, accounting for estimates from the finite-element models, the rule-of-mixture models, modified rule-of-mixture models, and the alternative models, the material properties for graphitereinforced composites will be taken to be those given in Table given below,
103 These properties can be considered to correspond to 65% fiber volume fraction. Properties for glass-reinforced polymer are taken from similar calculations for that material system. The important point to be aware of is that the material properties used throughout the book are consistent, starting at the micromechanics level with fiber and matrix properties. Learning Unit-2: M4.2 M4.2 Macromechanics of Laminae M4.2.1 Lamina Stress-Strain relations in material coordinates Historically, one of the most important assumptions regarding the study of the mechanics of fiber-reinforced materials is that the properties of the fibers and the properties of the matrix can be smeared into an equivalent homogeneous material with orthotropic material properties. If this assumption had not been made in the development of the mechanics of fiber-reinforced materials, very little progress would have been made in understanding their response. An equally important assumption in the development of the mechanics of fiber-reinforced materials is the plane-stress assumption, which is based on the manner in which fiber-reinforced composite materials are used in many structures. Specifically, fiber-reinforced materials are utilized in beams, plates, cylinders, and other structural shapes which have at least one characteristic geometric dimension an order of magnitude less than the other two dimensions. In these applications, three of the six components of stress are generally much smaller than the other three. With a plate, for example, the stresses in the plane of the plate are much larger than the
104 stresses perpendicular to that plane. In all calculations, then, the stress components perpendicular to the plane of the structure can be set to zero, greatly simplifying the solution of many problems. In the context of fiber-reinforced plates, for example (see Figure M4.2.1(a)), the stress components σ3, τ23andτ 13 are set to zero with the assumption that the 1-2 plane of the principal material coordinate system is in the plane of the plate. Stress components σ 1, σ 2 andτ 12 are considered to be much larger in magnitude than componentsσ3, τ23andτ 13. In fact, σ 1 should be the largest of all the stress components if the fibers are being utilized effectively. We use the term plane stress because σ 1, σ 2 andτ 12 lie in a plane, and stresses σ 3, τ 23 andτ 13 are perpendicular to this plane and are zero. The small element of Figure M4.2.1 (a) appears in Figure M4.2.1 (b) under the assumption of plane stress. Figure M4.2.1 (a) Stresses on a small element of fibre-reinforced material The plane-stress assumption can lead to inaccuracies, some serious and some not so serious. The most serious inaccuracy occurs in the analysis of a laminate near its edge. Laminates tend to come apart in the thickness direction, or delaminate, at their edges, much like common plywood. An understanding of this phenomenon, illustrated in Figure M , requires that all six components of stress be included in the analysis. It is exactly the stresses that are set to zero in the plane-stress assumption (i.e., σ3, τ23andτ 13 ) that are responsible for delamination, so an analysis that ignores these stresses cannot possibly be correct for a delamination study. Delaminations can also occur away from a free edge, with the layers separating in blister fashion. These are generally caused by the presence of imperfections between the layers. The out-ofplane stress components σ 3, τ 23 andτ 13 are also important in locations where structures or components of structures are joined together; Figures M and M illustrate some examples. Figure M shows a bonded joint consisting of two laminates subjected to tensile load P. For the load to be transferred from one laminate to the other, significant out-of-plane stresses, particularly shear, must develop in the laminates around the interface, as well as at the interface itself. As another example, in many situations stiffeners are used to increase the load capacity of plates, as in Figure M For the plate-stiffener combination to be effective, the plate must transfer some of the pressure load to the stiffener. Thickness direction stresses must develop in the plate and stiffener flange if load is to be transferred through the interface. In
105 general, all three components of out-of-plane stressσ3, τ23andτ 13 develop in this situation. Away from the stiffener the plate may be in a state of plane stress, so not only is there a region of the plate characterized by a fully three-dimensional stress state, there is also a transition region. In this transition region the conditions go from truly plane stress to a fully three-dimensional stress state, making the analysis of such a problem difficult and challenging. Figure M4.2.1 (b) Stresses acting on a small element of fiber-reinforced material in a state of plane stress Figure M4.2.1(c) Cube subjected to compression in 2-direction no constraints
106 Figure M Example of region of high out-of-plane stresses: Delamination at a free edge Figure M Another laminate Example of region of high out-of-plane stresses: Bonded joint Figure M Example of region of high out-of-plane stresses: Stiffened plate Figure M illustrates another area where through-the-thickness stresses are important. Often it is necessary, or desirable, to change the thickness of a laminate by gradually terminating some of the layers. Away from the terminated layer region each portion of the laminate could well be in a state of plane stress due to the applied inplane load P. However, the thicker region is in a different state of plane stress than the thinner region. To make the transition between the two stress states, three-dimensional effects occur.
107 The illustrations in Figures M M are prime examples of situations encountered in real composite structures. However, the plane-stress assumption is accurate in so many situations that one would be remiss in not taking advantage of its simplifications. The static, dynamic, and thermally induced deflections and the stresses that result from these, vibration frequencies, buckling loads, and many other responses of composite structures can be accurately predicted using the plane-stress assumption. What is important to remember when applying the planestress assumption is that it assumes that three stresses are small relative to the other three stresses and they have therefore been set to zero. They do not necessarily have to be exactly zero, and in fact in many cases they are not exactly zero. With the aid of the three-dimensional equilibrium equations of the theory of elasticity, calculations based on the plane-stress assumption can be used to predict the stress components that have been equated to zero. When these results are compared with predictions of the out-of-plane components based on rigorous analyses wherein the out-of-plane components are not assumed to be zero at the outset, we find that in many cases the comparisons are excellent. Thus, a plane-stress, or, using alternative terminology, a twodimensional analysis, is useful. Two of the major pitfalls associated with using the plane-stress assumption are: 1. The stress components equated to zero are often forgotten and no attempt is made to estimate their magnitude. 2. It is often erroneously assumed that because the stress component σ 3 is zero and therefore ignorable, the associated strain ε3 is also zero and ignorable. Figure M Example of region of high out-of-plane stresses: Region of terminal layers Regarding the former point, while certain stress components may indeed be small, the material may be very weak in resisting these stresses. As was stated earlier, a fiber-reinforced material is poor in resisting all stresses except stresses in the fiber direction. Thus, several stress components may be small and so the problem conforms to the plane-stress assumption. However, the out-of-plane stresses may be large enough to cause failure of the material and therefore they should not be completely ignored. Often they are. Regarding the second point, the stresses in the 1-2 plane of the principal material coordinate system can cause a significant strain response in the 3-direction. The assumption that ε3 is zero just because σ3 is negligible is wrong and, as we shall see shortly, defies the stress-strain relations that govern material behavior. It is important to keep these two points in mind as we focus our discussion in the following sections on the plane-stress condition.
108 M Stress-Strain Relations for Plane Stress To see why the plane-stress assumption is important, it is only necessary to see how it simplifies the stress-strain relations. Specifically, for the plane-stress assumptions σ3, τ23andτ 13 are set to zero in equations (M (a)) and (M (b)). Looking at equation (M (a)) first, we find, (M (a)) (M (b)) From this relation it is obvious that (M ) so with the plane-stress assumption there can be no shear strains whatsoever in the 2-3 and 1-3 planes. That is an important ramification of the assumption. Also, (M ) This equation indicates explicitly that for a state of plane stress there is an extensional strain in the 3-direction. To assume that strain ε3 is zero is absolutely wrong. That it is not zero is a direct result of Poisson's ratios ν13 and ν 23 acting through S13 ands 23, respectively, coupling with the
109 nonzero stress components σ 1 andσ 2. The above equation for ε 3 forms the basis for determining the thickness change of laminates subjected to inplane loads, and for computing through-thickness, or out-of-plane, Poisson's ratios of a laminate. Despite the fact that ε 3 is not zero, the plane-stress assumption leads to a relation involving only ε1, ε2, γ12andσ 1, σ 2, τ 12. By eliminating the third, fourth, and fifth equations of equation M (c), we find (M ) The definitions of the compliances have not changed from the tithe they were first introduced, namely, (M ) The 3x 3 matrix of compliances is called the reduced compliance matrix. In matrix notation the lower right hand element of a 3 x 3 matrix is usually given the subscript 33, though in the analysis of composites it has become conventional to retain the subscript convention from the three-dimensional formulation and maintain the subscript of the lower corner element as 66. For an isotropic material, equation (M ) reduces to (M ) If the plane-stress assumption is used to simplify the inverse form of the stress-strain relation, equation (M (b)), the result is
110 (M ) With the above, one also concludes that (M ) In analogy to equation (M ), the third equation of equation (M ) yields, (M ) Rearranged, it becomes (M ) This relationship also indicates that in this state of plane stress ε3 exists and equation ( ) indicates it can be computed by knowing ε 1 andε 2. The three-dimensional form equation (M ) cannot be reduced directly to obtain a relation involving onlyσ 1, σ 2, τ 12, in, and ε 1, ε 2, γ 12 by simply eliminating equations, as was done with equation (M (c)) to obtain equation (M ). However, equation (M ) can be used as follows: From equation (M ), the expressions for σ1and σ 2 are (M ) Substituting for ε3 using equation (M ) leads to
111 or (M ) Including the shear stress-shear strain relation, the relation between stresses and strains for the state of plane stress is written as (M ) The Qij are called the reduced stiffnesses and from equations (M ) and (M ) (M ) The term reduced is used in relations given by equations (M ) and (M ) because they are the result of reducing the problem from a fully three-dimensional to a two-dimensional,
112 or plane-stress, problem. However, the numerical values of the stiffnesses Q 11,Q 12, andq13 are actually less than the numerical values of their respective counterparts for a fully threedimensional problem, namely, C 11,C 12, and C 33 and so the stiffnesses are reduced in that sense also. It is very important to note that there is not really a numerically reduced compliance matrix. The elements in the plane-stress compliance matrix, equation (M ), are simply a subset of the elements from the three-dimensional compliance matrix, equation (M (c)), and their numerical values are the identical. On the other hand, the elements of the reduced stiffness matrix, equation (M ), involve a combination of elements from the three-dimensional stiffness matrix. It is absolutely wrong to write and claim this represents the reduced stiffness matrix. It simply is not so. By inverting equation (M ) and comparing it to equation (M ), it is clear that (M ) This provides a relationship between elements of the reduced compliance matrix and elements of the reduced stiffness matrix. A much more convenient form, and one that should be used in lieu of equation (M ), can be obtained by simply writing the compliance components in equation (M ) in terms of the appropriate engineering constants, namely,
113 (M ) This form will be used exclusively from now on. For an isotropic material the reduced stiffnesses become (M ) M Important Interpretation of Stress-Strain Relations Revisited When discussing general stress states, we strongly emphasized that only one of the quantities in each of the six stress-strain pairs σ1 ε1, σ2 ε2, σ3 ε3, τ 23 γ23, τ12 γ13 andτ12 γ12 could be specified. With the condition of plane stress, this restriction also holds. For the state of plane stress we assume that σ3, τ23,andτ13are zero. We can say nothing a priori regarding ε3, γ 23, andγ13- However, by using the stress-strain relations; we found, equation (M ), that is γ 23, andγ 13 are indeed zero. This is a consequence of the plane-stress condition, not a stipulation. The strain e3 is given by equation (M ), another consequence of the plane-stress condition. Of the three remaining stress-strain pairs, σ1 ε1, σ2 ε2,andτ12 γ12only one quantity in each of these pairs can be specified. The other quantity must be determined, as usual, by using the stress-strain relations, either equation (M ) or (M ), and the details of the specific problem being solved. M Numerical Results for the Plane-Stress Condition If in Figure M4.2.1 (a) the cube of material is subjected to only one stress ( σ 2 ), and all other stresses, that isσ 1 = σ 3 = τ 23 = τ 13 = τ 12 = 0, so the cube is in a state of plane stress. (M ) ε ε γ can Using the plane stress-strain relation equation (M ), we find the strains 1, 2,and 12 be determined directly as
114 (M ) The strain ε 3 must now be determined from the condition of equation (M ), now not a direct part of the stress-strain relations, but rather an auxiliary equation. From equation (M ) (M ) By knowing numerical values fors 12,S 22, ands 23, and using the definitions given below δδ 1 δδ 2 δδ ε 3 1 = ε 2 = ε 3 = Δ 1 Δ 2 Δ, 3 we can find the dimensional changes of the cube, by definitions given below, δδ 1 =Δ 1ε1 =Δ1S12σ2 δδ 2 =Δ 2ε2 =Δ2S22σ2 δδ =Δ ε =Δ S σ We can also find the dimensional change of the cube of Figure M (c) from the plane-stress stress-strain relations using equation (M ), though this approach is not as direct. In particular, for the stress state of Figure M (c), equation (M ) simplifies to (M ) From the first and third of these, (M ) and substituting into the second yields (M )
115 If equation (M ) is used, (M ) This equation seems that we have gone in circles we have not! What we have shown is that the plane-stress stress-strain relations yield results identical to the results obtained by using the general stress-strain relations if the problem is one of plane stress. This is an important point. If the problem is one of plane stress, then using the simpler forms, equations (M ) and (M ), rather than the more complicated forms, equations (M (a)) and (M (b)), gives the correct answer. The auxiliary conditions, either equation (M ) or (M ), can be used to obtain information about the strain 3 that is not a direct part of the plane-stress stress-strain relation. In that context, it is important to keep in mind that the out-of-plane engineering properties are still useful. For example, consider a layer of graphite-reinforced material 100 mm long, 50 mm wide, and mm thick. As shown in Figure M , this layer is subjected to a 3750 N inplane force in the fiber direction. The through-thickness strain in the layer can be calculated from equation (M ) and the numerical values ofs,s,s,s,s, S 23,S 44,S 55,andS 66, we can find values of strain ε 3. Figure M Layer subjected to inplane forces Note: In this module text in Italic indicates advanced concepts. Plane-Stress Stress-Strain Relations and the Effects of Free Thermal and Free Moisture Strains σ τ τ If a problem conforms to the plane-stress assumption, namely, 3 = 23 = 13 = 0, but free thermal moisture strains are important, then, starting with equation (M (b)),
116 ε α ΔT βδm S S S ε α ΔT β ΔM S S S ε α ΔT β ΔM S S S γ S γ S γ S σ 1 σ 2 σ 3 τ 23 τ 13 τ 12 = ( M (b) ) and following the same steps that led to equation (M ), we can conclude that (M ) which is identical to the case of no thermal or moisture expansion effects. This is a direct consequence of the conditionsτ 23 = τ 13 = 0. The conclusion regarding ε 3 is not exactly the same as the case with no free thermal or moisture strain effects, and in fact the conclusion is much more far reaching. Specifically, using the condition that σ 3 = 0 in equation (M (b)), we conclude that (M ) Equation (M ) will be the basis for determining the through-thickness, or out-of-plane, thermal or moisture expansion effects of a laminate. In this case the through-thickness strain does not depend solely on the through-thickness expansion coefficients α3or β 3. The throughthickness strain involves the compliances S 13 and S 23, which in turn involve the Poisson's ratios ν 13 and ν 23, as well as the inplane extensional moduli E 1 and E 2. This coupling of the throughthickness strain with the inplane and out-of-plane elastic properties leads to important consequences. More will be said of this later. Continuing with the development, we observe that the plane-stress stress-strain relations, including free thermal and moisture strain effects, become (M ) and
117 (M ) where the mechanical strains are given by (M (a)) σ C C C T M ε αδ βδ σ C C C T M 2 ε α Δ β Δ σ C C C α T β M 3 ε Δ Δ = ( M (b) ) τ C 0 0 γ τ C 0 γ τ C γ As in the three-dimensional stress-strain relations, equations (M (b)) and (M (b)), ε1, ε2, γ 12 above are the total strains. The dimensional changes are therefore given by (M ) not Equally important, ε3 in equation (M ) is the total strain. This is quite obvious when one considers that the right-hand side of that equation explicitly includes free thermal strain effects, free moisture strain effects, and stress-related effects. To continue with our examples of thermal deformations, consider a 50 mm x 50 mm x 50 mm element of material that is completely constrained in the 1- and 2-directions. To satisfy the
118 plane-stress condition, the element cannot be constrained in the 3-direction. The stresses in the two constrained directions and the deformation in the 3-direction due to a temperature increase of 50 C are to be determined. Moisture absorption is not an issue ( M = 0). For this case, because of the stated conditions, To determine the restraining stresses, equation (M ) is used to give (M ) (M ) To determine the deformation in the 3-direction, equation (M ) is used to yield (M ) where the various terms in equation (M ) are retained to show the interaction between two- and three-dimensional elastic properties, and the three coefficients of thermal expansion. Numerically, equations (M ) and (M ) giveσ 1, σ 2, τ 12, ε 3. The two sets of numbers indicates the effect of relaxing the constraint in the 3-direction. M4.2.2 Plane-Stress Stress-Strain Relations in a Global Coordinate System Introduction: One of the most important characteristics of structures made of fiber-reinforced materials, and one which dictates the manner in which they are analyzed, is the use of multiple fiber orientations. Generally structural laminates are made of multiple layers of fiber-reinforced material, and each layer has its own specific fiber orientation. To this point we have studied the response of fiber-reinforced materials in the principal material system, whether it is fully threedimensional stress-strain behavior, as in equations (M (a)) and ( (b)), or plane-stress behavior, as in equations (M ) and ( ). If we are to accommodate multiple layers of fiber-reinforced materials, each with its own fiber orientation, then we will be confronted with using multiple coordinate systems, each with its own orientation with respect to some global or structural coordinate system. If we are dealing with an x-y-z Cartesian coordinate system to describe the geometry of the structure, then the orientation of each principal material system must be defined with respect to the x-y-z system. If we are dealing with an x-θ-r
119 cylindrical coordinate system to describe the structure, then the orientation of each principal material system must be defined with respect to the x-θ-r system, and so forth, for a spherical coordinate system. This leads to a large number of coordinates systems and orientations for describing the response of the fiber-reinforced structure. As an alternative approach, we can refer the response of each layer of material to the same global system. We accomplish this by transforming the stress-strain relations from the coordinate system into the global coordinate system. This will be our approach here, in particular; it will be done for a state of plane stress using the standard transformation relations for stresses and strains learned in introductory strength-of-materials courses. Transformation can also be done for a general state of stress. However, transformation here will be limited to the plane-stress state because it will be useful for the development of classical lamination theory. Equally important, though, is the fact that the transformation of the description of the stress-strain response of fiber-reinforced material from the principal material coordinate system to a global coordinate system results in concepts so different from what one encounters with isotropic materials that it is best to start with a simpler plane-stress state and progress to the more complicated general stress state. When the concepts for the plane-stress stress state response described in a coordinate system other than the principal material coordinate system are fully understood, progression to a three-dimensional stress state is easier. ε 1 S S S σ ε 2 S S S σ ε 3 S S S σ γ S 0 0 τ γ S 0 τ γ S τ = ( M (a) ) σ 1 C C C ε σ 2 C C C ε σ 3 C C C ε τ C 0 0 γ τ C 0 γ τ C γ = ( M (b) ) M Transformation Relations
120 M Coordinate Transformation is Necessary The generalized Hooke's law of a fiber-reinforced lamina for the principal directions is not always the most convenient form for all applications. Usually, the coordinate system used to analyze a structure is based on the shape of the structure rather than the direction of the fibers of a particular lamina. For example, to analyze a bar or a shaft, we almost always align one axis of the coordinate system with the bar's longitudinal direction. However, the directions of the primary stresses may not line up with the chosen coordinate system. For instance, the failure plane of a brittle shaft under torsion is often at a 45 angle with the shaft. To fight this failure mode, layers with fibers running at ± 45 are usually added, resulting in a structure formed by laminae with different fiber directions. In order to "bring each layer to the same table," stress and strain transformation formulae are required. M Introduction to Transformation Relations Consider Figure M (a), the familiar picture of an isolated element in the principal material coordinate system. Figure M (b) shows a similar element but one that is isolated in an x-yz global coordinate system. The fibers are oriented at an angle θ with respect to the +x-axis of the global system. The fibers are parallel to the x-y plane and the 3- and z-axes coincide. The fibers assumed their orientation by a simple rotation of the principal material system about the 3- axis. The orientation angle θ will be considered positive when the fibers rotate counterclockwise from the +x-axis toward the +y axis. Often the fibers not being aligned with the edges of the element are referred to as an off-axis condition, generally meaning the fibers are not aligned with the analysis coordinate system (i.e., off the +x-axis). Although we will use the notation for a rectangular Cartesian coordinate system as the global system (i.e., x-y-z); the global coordinate system can be considered to be any orthogonal coordinate system. The use of a Cartesian system is for convenience only and the development is actually valid for any orthogonal coordinate system. The stress-strain relations are a description of the relations between stress and strain at a point within the material. The functional form of these relations does not depend on whether the point is a point in a rectangular Cartesian coordinate system, in a cylindrical coordinate system, or in a spherical, elliptical, or parabolic coordinate system. The stresses on the small volume of element are now identified in accordance with the x-y-z notation. The six components of stress and strain are denoted as
121 (M (c)) and the six components of stress are illustrated in Figure M Although we seem interested in describing the stress-strain relation in another coordinate system now that we have developed it and fully understand it in the system, we should emphasize that Figure M should be interpreted quite literally. We should interpret the figure as asking, "What is the relation between the stresses and deformations denoted in equation (M (c)) for a small volume of material whose fibers are oriented at some angle relative to the boundaries of the element rather than parallel to them?" This is the real issue! Loads will not be always applied parallel to the fibers; our intuition indicates that unusual deformations are likely to occur. The skewed orientation of the fibers must certainly cause unusual distortions of the originally cubic volume element. What are these deformations? How do they depend on fiber-orientation? Are they detrimental? Are they beneficial? Fortunately these and other questions can be answered by transforming the stress-strain relations from the system to the x-y-z system. Figure M Elements of fiber-reinforced material in and x-y-z coordinate systems
122 Figure M Stress components in x-y-z coordinate system If we consider the special case shown in Figure M (b), where the two coordinate systems are related to each other through a simple rotation θ about the z axis, then the stresses in the system are related to the stresses in the x-y-z system by (M ) For a state of plane stress, σ, τ andτ are zero, and upon rearranging, the third, fourth, and fifth components of equation (M ) give (M ) Because (M ) the only solution to the last two equations of equation (M ) is
123 (M ) leading to the conclusion that for a plane-stress state in the principal material coordinate system, the out-of-plane stress components in the x-y-z global coordinate system are also zero. This may have been intuitive but here we have shown it directly. The first, second, and sixth component of equation (M ) may look more familiar in the form (M ) This form is derivable from equation (M ) by using trigonometric identities and is the form usually found in introductory strength-of-materials courses. The form of equation (M ) will be most often used as it can be put in matrix form as (M ) This transformation matrix of trigonometric functions will be used frequently in the plane-stress analysis of fiber-reinforced composite materials and it will be denoted by [T], [T] being written as (M ) OR
124 (M ) where m = cosθ, n = sinθ. With the above notation equation (M ) can be written (M ) or (M ) The inverse of equation (M ) is, i.e., the coordinate transform of plane stress can be written in the following matrix form: (M ) OR (M ) which implies
125 (M ) OR (M ) In a similar manner, the strains transform according to the specialized relations equation (M ) as (M (a)) (M (b)) Note very well that the tensor shear strains,, not the engineering shear strains are being used in the above. These two measures of strain are different by a factor of two; that is,
126 (M ) If engineering shear strain is used instead, then the transformation relations become (M ) As a result of the plane-stress assumption, specifically by equation (M ), (M ) and by analogy to equation (M ), it is concluded from the fourth and fifth equation of equation (M ) that (M ) Also, due to the third equation of equation (M ) and equation (M ), (M ) More importantly, if equation (M ) is used to transform the stresses, then
127 This equation is very important because it indicates that a shear stress in the x-y planeτ xy produces an extensional strain, ε z perpendicular to that plane! For an isotropic material, S 13 = S 23, and this simply will not happen. Shear stresses do not cause extensional strains in isotropic materials! This generation of extensional strains by shear stresses is an important characteristic of fiber-reinforced composite materials. Returning to equation (M ) to focus on the strains involved in the plane-stress assumption, we can write the first, second, and sixth equations as (M ) or (M ) It is very important to note that the transformation retains the factor of with the engineering shear strain. M Transformed Reduced Compliance Continuing with the transformation of the stress-strain relations for plane stress to the x-y-z global coordinate system, the stress-strain relations in the principal material coordinate system, equation (M ), can be written in a slightly modified form to account for the use of the tensor shear strain rather than the engineering shear strain as
128 Using the transformations given by equations (M ) and (M ) in equation (M ) leads to (M ) and multiplying both sides of equation (M ) by [T] -1 results in (M ) Substituting for [T] and [T] -l from equations (M ) and (M ), we find that multiplying these three matrices together, and multiplying the third equation through by a factor of 2, yields (M ) OR
129 (M ) where the compliance matrix S or S ij is defined by, The S, is called to be as the transformed reduced compliances. Note that the factor of 1/2 ij has been removed and the engineering shear strain reintroduced. Equation (M ) is a fundamental equation for studying the plane-stress response of fiber-reinforced composite materials. The transformed reduced compliances are defined by (M ) OR
130 (M ) Equation (M ) and the definitions equation (M ) relate the strains of an element of fiber-reinforced material as measured in the x-y-z global coordinate system to the applied stresses measured in that coordinate system. We can look upon these equations as strictly the end result of simple steps in linear algebra, that is, transformations, inversions, and so forth. Alternatively, we can view them as what they actually are, namely, relations that describe what we shall see to be the complex response of an element of fiber-reinforced material in a state of plane stress that is subjected to stresses not aligned with the fibers, nor perpendicular to the fibers. The most profound results of equation (M ) are that a normal stress σ x will cause a shearing deformation γ xy through the S16 term, and similarly a normal stress ay will cause a shearing deformation through the S 26 term. Equally important, because of the existence of these same S16 and S 26 terms at other locations in the compliance matrix, a shear stress τ xy will cause strains ε x andε y. Such responses are totally different from those in metals. In metals, normal stresses do not cause shear strains, and shear stresses do not cause extensional strains. This coupling found in fiber-reinforced composites is termed shear-extension coupling. Shearextension coupling is an important characteristic and is responsible for interesting and important responses of fiber-reinforced composite materials. Recall, equation (M ) provided another example of shear-extension coupling. Through a series of examples we will examine the response of an element of fiber-reinforced material to simple stress states (i.e., σ x only, and then τ xy only) and compare the responses with the response of a similar element of metal. After we work through these specific examples, the implications and meaning of shear-extension coupling will be clear. Figure M shows the variations with θ of the various elements of the transformed reduced compliance matrix for a graphite-reinforced material. Note that S12 and all on-diagonal terms are even functions of θ, while the off-diagonal terms S16 and S 26 are odd functions of θ. The importance of this will be illustrated shortly. Also note the rapid variation of some of the compliances as θ increases or decreases from 0. At θ = 30, S11has increased by a factor of 8 relative to its value at θ = 0 and S 16 has changed from 0 at θ = 0 to nearly its maximum magnitude.
131 Figure M Variation of transformed reduced compliance with fiber angle θ for graphitereinforced composite Before proceeding with the examples, we should discuss two special cases of equation (M ). For the first case, consider the situation when the fibers are aligned with the x-axis, namely, θ = 0. With θ = 0, m = 1 and n = 0 and equation (M ) reduces to (M ) where the argument of 0 is used as a reminder that the S ij are functions of θ. The results of equation (M ) simply state that at θ = 0 the transformed reduced compliance degenerates to the reduced compliance, that is, the compliance in the principal material coordinate system. In the principal material system there is no S16 or S 26 - The quantities S 11, S 12, S 22,and S 66 are
132 often referred to as the on-axis compliances. The barred quantities of equation (M ) are frequently called the off-axis compliances. For the second special case, consider isotropic materials. The compliances of equation (M ) reduce to (M ) which can be demonstrated by using the definitions of the compliances for an isotropic material, equation (M ), in equation (M ). For example: (M (a)) (M (b)) But (M ) so (M )
133 The proof that (M ) is identical. From S 12, we see (M (a)) (M (b)) so by equation (M ) (M ) From S 16, we see (M (a)) (M (b)) Similarly it can be shown (M ) Finally,
134 (M (b)) Again, by equation (M ), (M ) Thus, independent of the direction of the coordinate system, for an isotropic material equation (M ) is true. We now turn to a series of examples that illustrate the shear-extension coupling predicted by the stress-strain relations of equation (M ), specifically the deformations caused by a tensile normal stress. Consider a thin element of aluminum subjected to a tensile stress σ x = 155 MPa. As in Figure M (a), me aluminum element has dimensions 50 mm x 50 mm. Thickness is not important at the moment but consider the element to be thin.
135 Figure M Response of aluminum and graphite-reinforced composite to tensile normal stress σ x As σ y and τ xy are zero, the stress-strain relations of equation (M ) reduce to (M ) or, by equation (M ),
136 (M ) Referring to Table M , we note that the strains in the aluminum are Table M Typical properties of several materials The dimensional changes of the square element of aluminum are
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
DESIGN OF LAMINATES FOR IN-PLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
A FINITE ELEMENT MODEL TO PREDICT MULTI- AXIAL STRESS-STRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
Delamination Studies in Fibre-Reinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
Composite Materials Fibre-Matrix Interfaces There is nothing there really except the two of you (or the fiber and matrix). Composite Parameters Fibre properties Composite Interfaces Matrix properties Fibre
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, firstname.lastname@example.org
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED - PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stress-strain diagram
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6-13-1, Ohsawa, Mitaka,
www.ijaser.com 2012 by the authors Licensee IJASER- Under Creative Commons License 3.0 email@example.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angle-ply FRP laminates
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto Gutierrez-Miravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLE-PLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
20 th International Conference on Composite Materials Copenhagen, 19-24 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFF-AXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
20 th International Conference on Composite Materials Copenhagen, 19-24th July 2015 Non-conventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 24-10-02
Chapter - Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205-212 (1991).
Stress-Strain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
, June 30 - July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
PROGRESSIVE FAILURE SIMULATION OF AS-MANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAIN-BASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475-477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
A Study on the Tube of Integral Propeller Shaft for the Rear-wheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmu-ro, Goesan-gun, South Korea.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & Free-Body Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR- Under Creative Commons License 3.0 firstname.lastname@example.org Research article
Basic Energy Principles in Stiffness Analysis Stress-Strain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
Aspect Ratio Requirements for Nanotube-Reinforced, Polymer-Matrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
A SELF-INDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK email@example.com
Lecture #10: 151-0735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 16-17 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a cross-sectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREE-DIMENSIONAL, TIME- DEPENDENT, NON-LINEAR, UNI-DIRECTIONAL
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
Bulk Properties of Solids Old Exam Questions Q1. The diagram shows how the stress varies with strain for metal specimens X and Y which are different. Both specimens were stretched until they broke. Which
International Journal of Mechanical Engineering and Technology (IJMET) Volume 8, Issue 5, May 2017, pp. 651 655, Article ID: IJMET_08_05_071 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=8&itype=5
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 15-16 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
MTS ADHESIVES PROGRAMME 1996-1999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to Visco-Elastic/Visco-Plastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO- AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 1229-1245. DOI: 10.1177/0021998305057432
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 5-22 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and Anne-Marie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS - Cachan, Avenue
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 79-85 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the three-dimensional analysis of compression molding
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., firstname.lastname@example.org Faculdade de Tecnologia de São Paulo, FATEC-SP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kip-in.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
SP-230 57 Strain-Based Design Model for FRP-Confined Concrete Columns by N. Saenz and C.P. Pantelides Synopsis: A constitutive strain-based confinement model is developed herein for circular concrete columns
5th International Symposium on NDT in Aerospace, 13-15th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
A Computer Simulation of Single Fiber Pull Out Process in a Composite WEN ZHONG AND NING PAN* Division of Textiles and Clothing Department of Biological and Agricultural Engineering University of California,
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
Concrete Technology Prof. B. Bhattacharjee Department of Civil Engineering Indian Institute of Technology, Delhi Lecture - 25 Strength of Concrete: Factors Affecting Test Results Welcome to module 6, lecture
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
Paper ID #15426 Using Mechanical Testing of Disposable Plastic Cups to Illustrate Processing- Structure-Property Relationships in an Introductory Materials Laboratory Course Dr. Kendra A. Erk, Purdue University